Review Layered Ternary and Quaternary Transition Metal Chalcogenide Based Catalysts for Water Splitting
Anand P. Tiwari 1,†, Travis G. Novak 1,†, Xiuming Bu 2, Johnny C. Ho 2,* and Seokwoo Jeon 1,*
1 Department of Materials Science and Engineering, KAIST Institute for the Nanocentury, Advanced Battery Center, KAIST, Daejeon 305-701, Korea; [email protected] (A.P.T.); [email protected] (T.G.N.) 2 Department of Materials Science and Engineering, City University of Hong Kong, 83 Tat Chee Avenue, Kowloon, Hong Kong; [email protected] * Correspondence: [email protected] (J.C.H.); [email protected] (S.J.); Tel.: +82-42-350-3342 (S.J.) † These authors contributed equally.
Received: 30 October 2018; Accepted: 13 November 2018; Published: 16 November 2018
Abstract: Water splitting plays an important role in the electrochemical and photoelectrochemical conversion of energy devices. Electrochemical water splitting by the hydrogen evolution reaction (HER) is a straightforward route to producing hydrogen (H2), which requires an efﬁcient electrocatalyst to minimize energy consumption. Recent advances have created a rapid rise in new electrocatalysts, particularly those based on non-precious metals. In this review, we present a comprehensive overview of the recent developments of ternary and quaternary 6d-group transition metal chalcogenides (TMCs) based electrocatalysts for water splitting, especially for HER. Detailed discussion is organized from binary to quaternary TMCs including, surface engineering, heterostructures, chalcogen substitutions and hierarchically structural design in TMCs. Moreover, emphasis is placed on future research scope and important challenges facing these electrocatalysts for further development in their performance towards water splitting.
Keywords: hydrogen; electrocatalysts; transition metal; layered material; heterostructure; hierarchical; surface engineering
1. Introduction In recent years, there has been increasing attention on renewable and environmentally friendly energy devices and energy sources as alternatives to fossil fuels [1,2]. In materials science research, two-dimensional (2D) layered materials such as graphene, transition metal chalcogenides (TMCs), MXenes and phosphorene have been heavily researched for many of these energy applications, including solar cells, batteries, light-emitting diodes, thermoelectric generators and so forth [3–8]. These layered 2D materials have also been studied as efﬁcient catalysts for the production of hydrogen, which has been proposed as the ideal energy carrier by virtue of its highest gravimetric energy density with zero emission of carbon dioxide [9,10]. Hydrogen is not available in free form but mainly exists in compounds such as hydrocarbons and water. At present, hydrogen is mainly produced from natural gas via steam reforming of hydrocarbons, which produces a large amount of greenhouse-gas emissions, making it neither renewable nor carbon-neutral . Therefore, current demand for hydrogen production is how to ﬁnd a sustainable, economical and large scale route. In this respect, hydrogen production via electrolytic or photocatalytic water splitting is highly desired for renewable and environmentally-friendly hydrogen production [1,12]. The water splitting reaction is possible through two different cathodic half electrochemical reactions: the oxygen evolution reaction (OER) and hydrogen evolution reaction (HER). HER activity is pivotal to a range of energy conversion devices including artiﬁcial photosynthetic cells.
Catalysts 2018, 8, 551; doi:10.3390/catal8110551 www.mdpi.com/journal/catalysts Catalysts 2018, 8, 551 2 of 29
HER activity proceeds through the reduction of protons accompanied be the subsequent evolution of gaseous hydrogen as follows: In acidic electrolytes: + 2H(aq) + 2e → H2(g) In alkaline electrolytes: − − 2H2O + 2e → H2(g) + 2OH(aq) The standard reduction potential of the HER is deﬁned versus a normal hydrogen electrode at pH = 0 as: 0 E + = 0 V H /H2O On top of the reduction potential, electrochemical processes have to surmount a certain activation energy barrier (known as overpotential) for water splitting activity to occur. Therefore, to promote the reaction rate and efﬁciency, HER activity demands the assistance of electrocatalysts to lower the overpotential [13,14]. In general, acidic electrolytes are more favorable because these units are more compact and could potentially run in reverse mode to produce electricity (i.e., in fuel cells) . To date the most effective catalysts for the HER activity under acidic conditions are the platinum group metals (PGMs, including Pt, Ru, Rh, Ir and Pd). Among PGMs, Pt is the most popular choice, which has a near-zero overpotential and is frequently used to benchmark the activity of other HER electrocatalysts . Nevertheless, the high price and shortage restrict the commercial application of PGMs for the HER electrocatalysts. Therefore, highly effective alternative HER electrocatalysts with good activity, high abundance and low cost  are key direction of research and two general strategies have been pursued. The ﬁrst one is to use microstructured or nanostructured electrocatalysts with a large surface area. This is because electrocatalysis is a surface process, meaning that structures with a high surface area can signiﬁcantly ease the demand on high catalyst loading . The second strategy is to make alloy PGMs with other metals, which can increase their active sites, allowing for lower catalyst loading . However, the non-homogeneous conﬁguration of nanostructures in PGMs restricts the stability towards electrocatalytic activity. Over the past decade, tremendous efforts have been actively made to replace the PGMs with many exciting advances [19,20]. In this regard, numerous earth-abundant compounds have been found to be competitive alternatives for PGMs, such as transition-metal dichalcogenides (MoS2, WS2, TaS2, etc.), transition metal carbides (WC, Mo2C, etc.) and transition metal phosphides (WP, MoP, etc.) for efﬁcient electrocatalysis towards water splitting [19,21]. Among the non-noble metal catalysts, layered transition-metal chalcogenides (TMCs) (MoS2, WS2) are promising because all of the catalytically active sites can be exposed due to atomically thin nature of 2D materials. Layered TMCs consist of alternating sheets of transition-metal atoms sandwiched between two chalcogen atoms . The difference in oxidation degree (for metal +4 and for chalcogen −2) causes the formation of strong ionic bonds between the metal and the chalcogen atoms that preserve the structure of the nanosheets, whereas the existence of weak van der Waals bonds between the individual layers enables the exfoliation of bulk crystals down to single layers . Moreover, a variety of compounds such as binary, ternary and quaternary TMCs with stoichiometric control of transition metals and chalcogens can provide us a rich platform to ﬁnd the best electrocatalyst to replace the noble metals for water splitting. How the variations in chemistry of the different layered TMCs compounds lead to dramatic differences in their catalytic activity is one of main theme of the article. Here we present a review on layered ternary and quaternary TMCs electrocatalysts with an emphasis on those made of 6d transition metals (Mo and W) and chalcogens (S and Se). First, we start with a brief introduction to water splitting electrocatalysis especially in acidic medium by thermodynamics and possible reaction pathways. Consequently, it is followed by detailed discussions on different TMCs based on their compositions: binary (contains one type of 6d transition metal and one type of chalcogen atoms), ternary (contains one type of 6d transition metal and two type of chalcogen atoms or two type of 6d transition metal and one type of chalcogen atoms) and Catalysts 2018, 8, 551 3 of 29 quaternary (contains two type of transition metal and two type of chalcogen atoms) electrocatalysts for water splitting in sequential order. For each type of electrocatalyst, we emphasize the morphology and structure control and its relationship with the electrocatalytic activities toward H2 production. Speciﬁcally, we summarize major achievements and discuss prevailing trends for improvement in the electrocatalytic activities by variation in atomic constituents. We also give a detailed overview on the recent progress of hierarchical structure design of TMCs. Finally, we present a perspective on the development of future research direction and challenges emerging from the layered TMCs nanomaterials towards water splitting electrocatalysts.
2. Electrochemistry and Hydrogen Evolution Reaction (HER)
2.1. Electrochemical Theory and Equations To understand the fundamentals of HER, Nernstian potential (under standard conditions) to a normal hydrogen electrode (NHE) is described by:
0 RT 1/2 EHER = E + − log αH+ /PH = −0.059 × (pH) V vs. NHE = 0 V vs. RHE (H2/H ) F 2 On the reversible hydrogen electrode (RHE) scale, the Nernstian potential for the HER is equal to zero regardless of electrolytes used. The HER activity does not start until a sufﬁcient cathodic potential is applied with reaction overpotentials . Taking this into consideration, the potential to drive the HER can be expressed as: Ei = EHER + iR + η where η is the reaction overpotential, which is one of the most important electrode parameters to evaluate its electrochemical performance. Overpotential at a speciﬁed apparent current density (normally at 10 mA/cm2 for HER) is a useful experimental parameter to characterize a given electrode in the working condition, whereas the onset overpotential, often namely as onset potential, refers to the smallest potential where the catalyst starts to catalytically function or the HER process begins. The smaller the overpotential, the higher the energy efﬁciency. Whereas iR is the ohmic potential drop caused by the ﬂow of current in the ionic electrolyte . The HER process consists of two primary steps in acidic electrolytes . The ﬁrst step known as the discharge reaction or Volmer reaction in which a proton-coupled electron transfer at the catalyst surface yields an intermediate adsorbed hydrogen atom :
+ + − → H(aq) e Hads
Furthermore, hydrogen desorption proceeds through two possible pathways. First, by electrochemical desorption reaction or Heyrovsky reaction in which the adsorbed hydrogen atom can react with another proton from the solution accompanied by a second electron transfer to form molecular hydrogen as:
+ + + − → Hads H(aq) e H2(g)
Another possible way for desorption of hydrogen is the recombination reaction or Tafel reaction in which two adsorbed hydrogen atoms form molecular hydrogen as :
Hads + Hads → H2(g)
To elucidate the operating mechanism on different HER electrocatalysts, the Tafel slope is taken as an indication of the rate determining step . It is deﬁned that the Tafel slope is 118 mV/dec, 39 mV/dec, or 29.5 mV/dec when the discharge reaction (Volmer reaction), the electrochemical desorption reaction (Heyrovsky reaction), or the recombination reaction (Tafel reaction) is rate determining, respectively. Catalysts 2018, 8, 551 4 of 29
It is clear from the above discussion that hydrogen adsorption and desorption on the electrode surface are two successive steps in HER electrocatalysis. However, hydrogen adsorption and desorption are competitive in nature. If catalyst surface has weak bonding strength with hydrogen atoms, it cannot efﬁciently adsorb the reactant to initiate the HER, whereas a catalyst surface having strong bonding strength would have difﬁculty in releasing the H2 toward the completion of the HER. Therefore, the ideal HER electrocatalysts should have well balanced hydrogen bonding and releasing properties . It is known that the maximum exchange current density is attained when hydrogen adsorption free energy is close to thermoneutral (i.e., ∆GH = 0). In this respect, Nørskov and co-workers calculated hydrogen adsorption free energy on different transition metals and plotted the HER exchange current density as a function of the calculated free energy . The plotted HER exchange current density as a function of the calculated free energy shows volcano-shaped curve with the peak position close to that of platinum. By following these results, they suggest that ∆GH is a useful descriptor in the selection of new electrocatalysts for hydrogen evolution. The intrinsic per-site activity of a catalyst is also an important metric for further improvement and to guide catalyst development, which is often measured by the turnover frequency (TOF) for each active site. TOF value is related to the activity of each catalytic site of the catalysts. The difﬁculty in measuring a TOF is not only in determining the rate but also in counting active sites because active sites may not be all identical even for the same catalyst. Practically, for different catalysts, the comparison of the TOFs is only meaningful when the value is taken at the same overpotential.
2.2. Experimental Conditions A common experimental setup for measuring HER activity is a three-electrode system . Here, the working electrode (the catalytic material being tested) is typically applied on a rotating disk, while the reference electrode is Ag/AgCl (or occasionally saturated calomel) and the counter electrode is Pt wire or graphite rod. To ensure the removal of dissolved oxygen, nitrogen bubbling is often continuously applied during measurements. This system allows for reliable testing of HER catalysts with a relatively simple system and a small amount of the tested material. However, it does not accurately reﬂect all of the challenges in the overall electrolysis of water. An alternative technique of water electrolysis is to use a polymer exchange membrane (PEM) instead of liquid electrolytes . PEM electrolyzers have the advantage of operating at high current densities and possessing more compact designs but suffer from issues due to higher operating pressures causing cross-permeation. Although this review will primarily focus on catalytic materials tested through the aforementioned three-electrode system, we note that the testing of HER catalysts in PEM electrolyzers is also an active research ﬁeld .
3. Non-Noble Transition Metals Based Electrocatalysts Generally, an ideal HER catalyst should be an earth-abundant material possessing good intrinsic material parameters of a near zero ∆GH and robust stability and extrinsic engineering parameters of the full utilization of catalytically active sites and efﬁcient charge transfer on the non-noble and earth-abundant materials. In this respect, nanostructures of non-noble metals materials and their heterostructures on the conducting support have been addressed for efﬁcient HER electrocatalysts [32,33]. Recently, transition metals alloys and their compounds have been investigated as a promising low-cost and non-noble metal material with high electrocatalytic performances. Within the past few years, transition metal carbides, borides and phosphides have been reported with very promising electrocatalytic activities [34–36]. In 2012, Xile Hu’s group have reported catalysts based on transition metal boride (i.e., MoB) and transition metal carbide (i.e., Mo2C) with efﬁcient electrocatalytic activity, which are able to rival non-noble metal HER performance working at pH = 0 . Moreover, transition metal carbide on conductive carbon nanotubes has shown good HER performance towards by solving the ion transfer problem in electrocatalytic activities . In addition, Shi et al. have reported chemical modiﬁcation of Mo2C via phosphorus doping for efﬁcient Catalysts 2018, 8, 551 5 of 29
electrocatalytic activity . Transition metal phosphides, such as Ni2P, FeP and Co2P, have also been reported for efﬁcient electrocatalytic activity in both acidic and alkaline electrolytes [40–43]. Other phosphides such as nanoparticles of WP and MoP are also showing great promise and recent reports indicate that they have overpotentials around 110 mV or even slightly below when freshly Catalysts 2018, 8, x FOR PEER REVIEW 5 of 29 prepared [44,45]. Another approach to get efﬁcient electrocatalysts for HER is to make hybrid structures containingmetals, carbon transition and nitrogen metals, carbon atoms and[46–48]. nitrogen Yin atomset al. [have46–48 ].reported Yin et al.Ni-C-N have reportednanosheets Ni-C-N with nanosheetsextremely high with performance extremely high electrocatalyst performance for electrocatalyst HER activity wherein for HER it activity is indicated wherein thatit overpotential is indicated thatis 61 overpotential mV or even slightly is 61 mV below, or even which slightly is benchmark below, which for isthe benchmark electrocatalytic for the activity electrocatalytic for HER activity. As formentioned HER [46 ].above, As mentioned there has above, been tremendous there has been progre tremendousss made progress in the field made of inacid-stable, the ﬁeld of nonprecious acid-stable, nonpreciousHER catalysts HER in the catalysts past few in years, the pastillustrated few years, by Figure illustrated 1, which by shows Figure selected1, which highlights shows selected from the highlightsrecent literature. from the recent literature.
FigureFigure 1.1. ChronologicalChronological trendtrend inin overpotentialoverpotential atat currentcurrentdensity densityof of 10 10 mA mA cm cm−−22 ofof somesome reportedreported earth-abundantearth-abundant transition transition metal metal based based catalysts catalysts along withalong the with Pt/C the catalyst Pt/C (experimentally catalyst (experimentally measured).
Notemeasured). that all Note catalysts that shown all catalysts here were shown measured here inwere 0.5 Mmeasured H2SO4 to in ensure 0.5 M a H fair2SO comparison.4 to ensure a fair comparison. 4. Layered Transition Metal Chalcogenides 4. LayeredOver the Transition last decade, Metal transition Chalcogenides metalchalcogenides (TMCs) have gained growing attention for manyOver applications the last decade, such transition as electrocatalysts. metal chalcoge To maximizenides (TMCs) the electrocatalytic have gained growing properties attention of TMC for materials,many applications there are twosuch primary as electrocatalysts. approaches: increasingTo maximize the numberthe electrocatalytic of active sites properties through structural of TMC engineeringmaterials, there (extrinsic) are two and primary modifying approaches: the chemical increasi compositionng the number to of reduce active the sites∆G throughH (intrinsic) structural . By changing the structures and compositions (intrinsic and extrinsic) of TMCs, a variety of compounds engineering (extrinsic) and modifying the chemical composition to reduce the ΔGH (intrinsic) . By withchanging different the transitionstructures metalsand compositions and chalcogens (intrinsic can be and realized. extrinsic) Here of we TMCs, present a variety three differentof compounds types ofwith TMCs: different binary, transition ternary metals and quaternary. and chalcogens can be realized. Here we present three different types 4.1.of TMCs: Binary binary, Transition tern Metalary and Chalcogenides quaternary.
4.1. BinaryBinary Transition TMCs are Metal mostly Chalcogenides known as transition metal dichalcogenides (TMDs), which contain one type transition metal and one type of chalcogen in their chemical formula. The most well-known Binary TMCs are mostly known as transition metal dichalcogenides (TMDs), which contain one example among them is MoS . MoS naturally occurs as a lamellar hexagonally structure similar type transition metal and one2 type of2 chalcogen in their chemical formula. The most well-known to graphite in which the individual S−Mo−S layers weakly interact with each other by van der example among them is MoS2. MoS2 naturally occurs as a lamellar hexagonally structure similar to Waals forces and each layer has a thickness of ~0.64 nm (shown in Figure2a) [ 50,51]. Normally, graphite in which the individual S−Mo−S layers weakly interact with each other by van der Waals MoS2 occurs in two different phases, 2H and 1T. The hexagonal 2H polytype has two layers per forces and each layer has a thickness of ~0.64 nm (shown in Figure 2a) [50,51]. Normally, MoS2 occurs unit cell along the c-axis and 1T-polytype has trigonal in nature, the 2H-type is dominant and more in two different phases, 2H and 1T. The hexagonal 2H polytype has two layers per unit cell along the c-axis and 1T-polytype has trigonal in nature, the 2H-type is dominant and more stable and 1-T can synthesized by 2H phase heating (shown in Figure 2a) . There are many methods have been employed to prepare single- and multi-layer binary TMCs. The top-down methods to create 2D materials, which rely on the exfoliation of layered bulk crystals to make few layer flakes, include the mechanical cleavage method , chemical intercalation and exfoliation [54–56] electrochemical intercalation and exfoliation , liquid phase exfoliation by direct sonication in solvents .
Catalysts 2018, 8, 551 6 of 29
stable and 1-T can synthesized by 2H phase heating (shown in Figure2a) [ 52]. There are many methods have been employed to prepare single- and multi-layer binary TMCs. The top-down methods to create 2D materials, which rely on the exfoliation of layered bulk crystals to make few layer Catalystsﬂakes, 2018 include, 8, x FOR the PEER mechanical REVIEW cleavage method , chemical intercalation and exfoliation [546 of– 5629] electrochemical intercalation and exfoliation , liquid phase exfoliation by direct sonication in Examplessolvents [ 52of]. bottom-up Examples ofapproaches bottom-up are approaches chemical are vapor chemical deposition vapor deposition(CVD) growth (CVD) [58–60] growth and [58 wet–60] chemicaland wet chemicalsynthesis synthesistechniques, techniques, such as hydrothermal such as hydrothermal reactionsreactions . .
FigureFigure 2. 2. (a(a) )Schematic Schematic illustration illustration of of the the 2H-type 2H-type structure structure of ofbinary binary MoS MoS2 and2 and 1T-type 1T-type structure structure of
binaryof binary MoS MoS2. Reprinted2. Reprinted with with permission permission from from Reference Reference , [52 ],copyright copyright (2013), (2013), Royal Royal Society Society of of Chemistry.Chemistry. ( (bb)) Top Top and and side side views views of of the the optimized optimized geom geometryetry of of two two anion anion contains contains ternary ternary MoSSe MoSSe
andand atomic atomic structures of twotwo cationcation containscontains ternaryternary MoMo1−1−xWWxxSS2 2atomicatomic structures. structures. Reprinted Reprinted with with permissionpermission from from Reference Reference , , copyright copyright (2018), (2018), American American Chemical Chemical Society Society and and Reference Reference , , copyrightcopyright (2017), (2017), Scientific Scientiﬁc Reports. (c) LayeredLayered andand crystalcrystal structurestructure of of quaternary quaternary Cu Cu2Mo(S2Mo(S1−1−ySeSeyy))44. . ReprintedReprinted with with permission permission from from Refe Referencerence , , copyright copyright (2016), (2016), Elsevier. Elsevier. 4.2. Ternary Transition Metal Chalcogenides 4.2. Ternary Transition Metal Chalcogenides There are two type of ternary TMCs possible, the ﬁrst contains two types of transition metal and There are two type of ternary TMCs possible, the first contains two types of transition metal and one type of chalcogen in their chemical formula, while the other type contains one transition metal one type of chalcogen in their chemical formula, while the other type contains one transition metal and two types of chalcogen in their chemical compositions. By tuning the atomic ratio of transition and two types of chalcogen in their chemical compositions. By tuning the atomic ratio of transition metals or chalcogen atoms, researchers have found interesting tunable electronic and optical properties, metals or chalcogen atoms, researchers have found interesting tunable electronic and optical which would be useful for water splitting electrocatalysts. Recently, Guan et al. have reported ternary properties, which would be useful for water splitting electrocatalysts. Recently, Guan et al. have MoSSe materials, which have semiconductor properties with a direct band gap of 2.14 eV. By theoretical reported ternary MoSSe materials, which have semiconductor properties with a direct band gap of calculation, it is found that MoSSe holds an appropriate band edge alignment with the water redox 2.14 eV. By theoretical calculation, it is found that MoSSe holds an appropriate band edge alignment potentials. The crystal structure of MoSSe is a compromise of binary TMCs MoS2 and MoSe2 (shown in with the water redox potentials. The crystal structure of MoSSe is a compromise of binary TMCs MoS2 Figure2b) [ 62]. Zhang group has reported the synthesis of MoSSe by simple CVD method, which shows and MoSe2 (shown in Figure 2b) . Zhang group has reported the synthesis of MoSSe by simple extraordinary results in terms of electronic properties . However, MoS − Se2x and WS − Se2x CVD method, which shows extraordinary results in terms of electronic 2(1propertiesx) . However,2(1 x) alloy nanoﬂakes have been synthesized by simple solvothermal process [66,67]. Meanwhile, the Jeon MoS2(1−x)Se2x and WS2(1−x)Se2x alloy nanoflakes have been synthesized by simple solvothermal process group has reported synthesis of MoSXOy by simple CVD method to modulation of band structures [66,67]. Meanwhile, the Jeon group has reported synthesis of MoSXOy by simple CVD method to of MoS2 . The Fan group has analyzed other type of ternary TMCs that contain two type of modulation of band structures of MoS2 . The Fan group has analyzed other type of ternary TMCs transition metal, in which they have shown different ordered and disordered phases of Mo1−xWxS2 that contain two type of transition metal, in which they have shown different ordered and disordered monolayer . phases of Mo1−xWxS2 monolayer . 4.3. Quaternary Transition Metal Chalcogenides 4.3. Quaternary Transition Metal Chalcogenides Quaternary TMCs contain two types of transition metal and two types of chalcogen in their chemicalQuaternary formula. TMCs Quaternary contain TMCstwo types can beof easilytransiti synthesizedon metal and by atwo solvothermal types of chalcogen method inin which their chemicalone chalcogen formula. atoms Quaternary are replaced TMCs by othercan be type easily of chalcogensynthesized atoms by a insolvothermal the structures. method TheLee in which group one chalcogen atoms are replaced by other type of chalcogen atoms in the structures. The Lee group have synthesized monolayer of Cu2Mo(SySe1−y)4 quaternary TMC by a solution processed method for have synthesized monolayer of Cu2Mo(SySe1−y)4 quaternary TMC by a solution processed method for extraordinary electrocatalytic activity . The structure of quaternary TMCs can be viewed as layers of transition metals and chalcogen atoms as shown in Figure 2c; the layers are perpendicular to the c direction. Similar to binary TMCs, atoms within the layers of quaternary TMCs are covalently bound, while there are only van der Waals interactions between the layers . Another description of the structure of quaternary TMCs follows from the recognition that the chalcogen lattice can be viewed as a distorted cubic close-packed array of chalcogen atoms (shown in Figure 2c). The two-dimensional
Catalysts 2018, 8, 551 7 of 29 extraordinary electrocatalytic activity . The structure of quaternary TMCs can be viewed as layers of transition metals and chalcogen atoms as shown in Figure2c; the layers are perpendicular to the c direction. Similar to binary TMCs, atoms within the layers of quaternary TMCs are covalently bound, while there are only van der Waals interactions between the layers . Another description of the structure of quaternary TMCs follows from the recognition that the chalcogen lattice can be viewed as a distorted cubic close-packed array of chalcogen atoms (shown in Figure2c). The two-dimensional structure results from transition metal atom occupation of 3/4 of the tetrahedral holes in alternating layers along the c direction; only 3% of the total number of tetrahedral holes are ﬁlled.
5. Layered Transition Metal Chalcogenides Based Electrocatalysts for HER In 2005, Nørskov et al. applied density functional theory (DFT) calculations to analyze the free energy of hydrogen bonding (∆GH*) to layered binary TMC MoS2, which revealed that while the basal plane of MoS2 is catalytically inert, its sulﬁde Mo-edges are active for the HER with suitable ∆GH* = 0.1 V, close to those of several efﬁcient HER electrocatalysts including Pt, nitrogenase and hydrogenase . The theoretical results are conﬁrmed with their experimental ﬁndings, that shows nanosized MoS2 clusters on a graphite support indeed have very decent HER activity with an overpotential in the range of 0.1–0.2 V at pH = 0 . The theoretical results show that the best edge conﬁgurations correspond to Mo edges covered by 50% S with ∆GH* = 0.06 eV compared to S edges covered by 100% S: ∆GH* = −0.45 eV (shown in Figure3a) [ 71]. Similar to MoS2, WS2 edges have also been found to be active with ∆GH* = −0.04 and −0.06 eV for 50% W edges and 100% S edges, respectively. Additional insights about the active sites (notably the importance of edge sites) can be obtained through spectroscopic techniques. Lassallee-Kaiser et al.  used X-ray absorption spectroscopy (XAS) and MoS3 in an acidic environment to assert that Mo(III) units with terminal disulﬁde ligands are the primary active site in MoS2 and that protonation and reduction of the outer S2 sites is the rate-limiting step for HER. However, some recent works have disputed this conclusion and argued (based on ∆GH calculations) that Mo-edges are more energetically favorable than S-edges for catalytic activity in pristine MoS2, while noting that in cases of doped MoS2 both Mo and S edges contribute to HER activity [73,74]. Regardless of the precise mechanism, it is clear that the identiﬁcation and promotion of edge sites is critical for catalyst development. In MoS2, this can be estimated through 1 Raman spectroscopy, where increased intensity of the A g out-of-plane mode often indicates additional exposed edge sites [75,76]. Jaramillo et al., who correlated the electrochemical activity and edge length of MoS2 nanoclusters measured by STM, obtained experimental evidence on the crucial role of edges in the HER (Shown in Figure3b) [ 77]. Experimentally, exchange current density per active site and the turnover frequency (TOF) (the number of hydrogen molecules/atoms per second being produced per active site per −1 −1 second) for MoS2 edges reaches 0.02 s for compared with 0.9 s for Pt (111) and rapidly increases with the overpotential (summarized in Figure3c). Moreover, other sulfur and selenium based TMCs from group 6d transition metal follow same trends as MoS2 and WS2 . The stability of active sites is important for electrocatalysis process. The stability of edges or the basal planes of TMCs are predicted from calculation of adsorption energy of hydrogen on the chalcogen atoms (∆GH−x, X = S, Se). Tsai et al. calculated the free energy of hydrogen adsorption on chalcogen atoms to estimate the catalytic activity and the stability of the edges and basal planes of various TMCs (shown in Figure3e,f) [ 78]. The values of adsorption energy reveals that the stability with activity on the basal plane is signiﬁcantly lower in the case of metallic TMCs compared with that of semiconducting TMCs. However, the results indicate that the basal planes of TMCs can be catalytically activated for metallic TMCs with lower free energy of hydrogen adsorption, which open new avenues for improving the HER activity of layered TMCs. Catalysts 2018, 8, 551 8 of 29 Catalysts 2018, 8, x FOR PEER REVIEW 8 of 29
FigureFigure 3. (3.a) ( Moleculara) Molecular model model of of a a platelet platelet exposingexposing both both Mo Mo and and S-edges S-edges from from top top and and side side view. view. ReprintedReprinted with with permission permission fromfrom , , copy copyrightright (2014), (2014), American American Chemical Chemical Society. Society. (b) STM ( bon) MoS STM2 on MoSnanoplatelets2 nanoplatelets on onAu Au(111). (111). Reprinted Reprinted with with perm permissionission from from Reference Reference , [77 copyright], copyright (2007), (2007), AmericanAmerican Association Association for for the the Advancement Advancement of of Science. Science. Thermodynamics Thermodynamics of of hydrogen hydrogen adsorptionadsorption on 2D transition2D transition metal metal dichalcogenides. dichalcogenides. (c) Sabatier (c) Sabatier “volcano” “volcano” plot plot showing showing the the exchange exchange currentcurrent density density as
a functionas a function of free of energy free energy of hydrogen of hydrogen adsorption adsorption of free-standing of free-standing (FS) (FS) MoS MoS2 edges,2 edges, MoS MoS2 2edges edges onon Au Au (111), MoS2 edges on graphene, vertically grown Fe, Cu, Ni, Co-promoted MoS2 edges, vertically (111), MoS2 edges on graphene, vertically grown Fe, Cu, Ni, Co-promoted MoS2 edges, vertically grown grown MoS2 edges, vertically grown MoSe2 edges, 1T WS2 basal plane and compared with various MoS2 edges, vertically grown MoSe2 edges, 1T WS2 basal plane and compared with various metals. (d) Evolutionmetals. (d of) Evolution turnover frequencyof turnover of severalfrequency catalysts of seve basedral oncatalysts transition-metal based on chalcogenidestransition-metal with chalcogenides with overpotential. (e,f) Plots of ΔGH*: the free energy of hydrogen adsorption as overpotential. (e,f) Plots of ∆GH*: the free energy of hydrogen adsorption as function of ∆GHX (X = S function of ΔGHX (X = S or Se): the HX adsorption free energy. (e,f) The evolution is displayed for or Se): the HX adsorption free energy. (e,f) The evolution is displayed for metallic TMDs (e) and metallic TMDs (e) and semiconducting TMDs (f). In general the stronger binding of X (ΔGHX < 0), the semiconducting TMDs (f). In general the stronger binding of X (∆GHX < 0), the higher stability of higher stability of TMDs, the lower the reactivity of TMDs (ΔGH* > 0), the weaker the hydrogen TMDs, the lower the reactivity of TMDs (∆G * > 0), the weaker the hydrogen binding. Reprinted with binding. Reprinted with permission from ReferenceH , copyright (2016), Wiley-VCH. permission from Reference , copyright (2016), Wiley-VCH.
Catalysts 2018, 8, 551 9 of 29
6. Materials Engineering for Improving Electrocatalytic Activity of TMCs
6.1. Edge and Defect Engineering to Enhance the Electrocatalytic Activity of TMCs The study of electrochemical activities of TMC edges has opened a new path for increasing the catalytic performances by optimizing the basal plane to edge ratio. In this respect, Xie’s group have developed defect-rich MoS2 nanosheets (Figure4a) and highlighted that their MoS 2 sheets contained abundant defects, which resulted in partial cracking of the catalytically inert basal planes, leading to the exposure of additional active edge sites (Figure4a) [ 80,81]. The as-obtained defect-rich MoS2 sheets shows an excellent HER activity with an onset potential of 0.12 V versus RHE and a Tafel slope of 50 mVdec−1, as well as a prominent electrochemical durability (Figure4a). However, it is known that the resistivity through the basal planes of layered multi-layer MoS2 has been measured to be 2200 times larger as compared to the value along the single layer MoS2 nanosheets, which leads to decrease the electrocatalytic activity with increase the number of layers of MoS2 . Yu et al. have reported that the catalytic activity of MoS2 decreases by 4.5 times when adding a layer of MoS2 due to the large potential required for electron hopping between successive layers (shown in Figure4b) [ 83]. However, synthesizing vertical or mesoporous MoS2 can tackle the challenge of layer dependence and utilization of active edge sites for electrocatalytic activity. Jaramillo et al. have reported contiguous large-area thin ﬁlms of a highly ordered double gyroid MoS2 network by templating mesoporous silica ﬁlms . The as-synthesized highly ordered double gyroid MoS2 exhibits an HER onset overpotential of 150–200 mV and a Tafel slope of 50 mV per decade. However, Cui et al. have demonstrated vertically aligned MoS2 ﬁlms by a rapid sulfurization process to convert Mo thin ﬁlms deposited on various substrates . The vertically aligned MoS2 ﬁlms show excellent electrocatalytic activity with a large exchange current density of 2.2 × 10−6 A cm−2 and a TOF = 0.013 s−1.
6.2. Support of Conducting Material to Improve Catalytic Activity of TMCs The conducting support materials can inﬂuence the energy of hydrogen adsorption for TMCs . Normally, if the binding between conducting material and TMCs is strong then hydrogen adsorption will be weak. Tsai et al. have calculated the free energy of hydrogen adsorption for MoS2 supported on various conducting substrates, such as gold, graphene and MoS2, which shows that ∆GH* for the Mo edge on graphene or gold is signiﬁcantly higher compared to the freestanding Mo-edge . Although ∆GH* reveals useful insights for HER electrocatalytic activity, it provides only a partial picture of HER process at the heterostructures of conducting substrate and TMCs . The electrical conductivity is an important parameter to enhance electrocatalytic activities. In poorly conducting materials, an additional potential is required to drive electrons more efﬁciently to the active sites for electrocatalytic activity. This is a major drawback for group 6d TMCs, which typically consist of a semiconducting trigonal prismatic structure. The intrinsic conductivity 6d TMCs can be enhanced via doping or by growing the nanosheets on a conducting surface. Li et al. have synthesized MoS2 nanoparticles on the conducting reduced graphene oxides (r-GO) surface . As seen in Figure4c,d, the introduction of rGO enhances signiﬁcantly catalytic activity of MoS2, showing a small onset potential of 0.1 V versus RHE and a low Tafel slope of 41 mV dec−1. Similarly, Yang et al. have reported a layered WS2 on rGO with enhanced electrocatalytic activity . The growth of TMCs on graphene enables a strong anchoring of nanosheets on the graphene basal plane, which improves the electrical conductivity and leads to a dramatic decrease of the charge-transfer resistance . Efforts have been made to enhance electrocatalytic activity of TMCs by materials engineering via making heterostructures and different architectures of TMCs but structural instability and difﬁculty in correlation of morphology control or atomic scale modiﬁcation with improved HER activity make the strategy less useful . Catalysts 2018, 8, 551 10 of 29 Catalysts 2018, 8, x FOR PEER REVIEW 10 of 29
FigureFigure 4.4. (a(a)) Schematic Schematic representation representation of defect-richof defect-rich MoS 2MoSnanosheets2 nanosheets and polarization and polarization curves obtained curves obtainedfrom MoS from2 nanosheets MoS2 nanosheets with various with densities various of densities defects. Reprinted of defects. with Reprinted permission with from permission Reference from , Referencecopyright , (2013) copyright Wiley-VCH. (2013) (b) Wiley-VCH. Schematic illustrating (b) Schematic the electron illustrating hopping the electron between hopping the layers between of MoS2 theand layers evolution of MoS of2 the and exchange evolution current of the densityexchange of current MoS2 with density increasing of MoS number2 with increasing of layers. number Reprinted of layers.with permission Reprinted with from permission Reference [from83], copyright Reference (2014), , copyright American (2014), Chemical American Society. Chemical (c) Illustration Society.
(forc) Illustration the MoS2 nanoparticlesfor the MoS2 nanoparticles decoration on decoration conductive on conductive graphene layer. graphene (d) Tafel layer. plots (d) Tafel for the plots MoS for2
thenanoparticles MoS2 nanoparticles and MoS and2 nanoparticles MoS2 nanoparticles decorated decorated graphene graphene samples samples along along with Pt.with Reprinted Pt. Reprinted with withpermission permission from from Reference Reference , copyright, copyright (2011), (2011), American American Chemical Chemical Society. Society. 6.3. Design of Hierarchical Structure to Further Improve the Catalytic Activity of TMCs 6.3. Design of Hierarchical Structure to Further Improve the Catalytic Activity of TMCs In principal, the further performance improvement of catalysts can be achieved in two aspects, In principal, the further performance improvement of catalysts can be achieved in two aspects, which include the increase of their intrinsic activity of single/multi-active sites and the upturn which include the increase of their intrinsic activity of single/multi-active sites and the upturn of their of their surface area. The former one has been discussed above through the synergistic effect surface area. The former one has been discussed above through the synergistic effect among among multicomponents towards the adjustment of their active sites. The latter one can be multicomponents towards the adjustment of their active sites. The latter one can be achieved by achieved by increasing the exposure surface area of catalysts in the electrolyte. Normally, the higher increasing the exposure surface area of catalysts in the electrolyte. Normally, the higher surface-to- surface-to-volume ratio is favorable for exposing the active sites. However, the agglomerated volume ratio is favorable for exposing the active sites. However, the agglomerated nanoparticles nanoparticles often bring alone adverse effects on the electrocatalytic performance, for instance the low often bring alone adverse effects on the electrocatalytic performance, for instance the low utilization utilization of catalysts and high charge transfer resistance. Simultaneously, the coated electrocatalyst of catalysts and high charge transfer resistance. Simultaneously, the coated electrocatalyst layer on layer on the electrode is prone to peel off from the substrate during vigorous gas evolution under the electrode is prone to peel off from the substrate during vigorous gas evolution under a high a high current density, which signiﬁcantly limits the practical applications. Hence, the design and current density, which significantly limits the practical applications. Hence, the design and synthesis synthesis of hierarchical structure is necessary that can solve the above problems effectively by offering of hierarchical structure is necessary that can solve the above problems effectively by offering a a seamless integration. At the same time, the use of hierarchical structure also provides many other seamless integration. At the same time, the use of hierarchical structure also provides many other advantages, such as improving the penetration of electrolyte and releasing gas bubbles efficiently because of the associated increasing amount of free space there.
Catalysts 2018, 8, 551 11 of 29 advantages, such as improving the penetration of electrolyte and releasing gas bubbles efﬁciently because of the associated increasing amount of free space there. Particularly, hierarchically nanostructured NiFeSe can be prepared as an efﬁcient OER catalyst using Prussian blue as the template . The preparation process is divided into two steps. Ni-Fe Prussian blue analog is ﬁrst etched via ammonia and then followed by selenylation at N2 atmosphere. As chemical etching time increases, the morphologies evolve from nanocubes and nanodisks to nanocages, as seen in Figure5a. The ﬁnal product of NiFeSe nanocages shows the excellent OER performance that affords a current density 10 mA/cm2 at a small overpotential of 240 mV. The excellent performance can be attributed to the larger electrochemically active surface area, which beneﬁts from the high electrolyte-catalyst contact interface area provided by the open and hollow structure. Typically, the hierarchical structure can be mainly divided into three categories, including the polyhedral shape with special structures (e.g., star-shaped, concave tetrahedral, etc.), the unusual morphological features formed via the interaction of nanoparticles (e.g., core-shell, segments and branches, etc.) and the integration of multiple dimensional subunits in the nanoscale (e.g., zero dimensional nanoparticles, one dimensional nanowires or nanotubes, two dimensional nanosheets, etc.). Until now, there are many excellent reviews on the design of hierarchical structure [90–92]. In terms of TMC served as electrocatalysts, most of the hierarchical structure are belonged to the third conﬁguration discussed above, in which they are mostly prepared via the solvothermal method. In this regard, the following section will particularly focus on the recent research progress of hierarchical structure from the perspective of solvothermal synthesis.
6.4. Support/Template Synthesis for Hierarchical Structures The preparation of hierarchical structure by template-assisted methods can be rather straightforward in the concept. In general, the template-assisted synthesis can be divided into three kinds, in which they are the hard-template method, soft-template and self-template schemes. For the hard-template method, the introduced template with high uniformity is usually employed as physical scaffolds to create continuous voids in the ﬁnal product, which can be subsequently removed. Speciﬁcally, there are four key steps involved: (1) template preparation, (2) template surface functionalization, (3) target material coating and (4) template removal. Typical hard template materials consist of SiO2, carbon sphere, anodized aluminum oxide (AAO), metal-based structures with speciﬁc shapes, 2D materials and many others. For example, multiscale MoS2 foam was successfully prepared by using SiO2 as the hard template . Detailed TEM characterization reveals that the MoS2 foam possess abundant spherical voids, where MoS2 nanosheets are also vertically aligned around the mesopores with a large fraction of edge sites exposed. This study can evidently demonstrate many advantages of hierarchical structure via overall consideration of the mass transport and the accessibility towards HER. Besides, hierarchical transition-metal dichalcogenide nanosheets can as well be prepared from 2D nanosheets. Zhang’s group reported the hierarchical TMC nanosheets (MoS2 and WS2) via a one-pot heating treatment of melamine and metal precursors, as seen in Figure5b [ 94]. At ﬁrst, the polymerization of melamine into carbon nitride during thermal treatment can direct the horizontal growth of TMD nanoplates. Then, the subsequent decomposition of carbon nitride can guide the vertical growth of hierarchical TMC nanosheets. In any case, although uniform shapes and morphologies of the hierarchical structure can be readily prepared via hard-template methods, the tedious and complex preparation process would limit their practical applications. Importantly, homogeneous nucleation often takes precedence over heterogeneous nucleation on the surface of the template in solution, which would eventually induce the failure of the warp structure. Catalysts 2018, 8, 551 12 of 29
Catalysts 2018, 8, x FOR PEER REVIEW 12 of 29
Figure 5.5. ((aa)) The The evolution evolution of of hierarchical hierarchical Ni-Fe-Se Ni-Fe-Se nanocages prepared via chemical etching. Reprinted with permission from ReferenceReference [,89], copyright (2017), Wiley-VCH. (b) ProcedureProcedure ofof hierarchical TMC nanosheets using carbon nitride asas thethe template.template. Reprinted with permissionpermission from Reference [,94], copyrightcopyright (2015),(2015), Wiley-VCH. Wiley-VCH. ( c()c) Hierarchical Hierarchical MoS MoS2/NiCo2/NiCo22SS44/CFP structure structure prepared via anion-exchangeanion-exchange reaction. reaction. Reprinted Reprinted with with permission permission from Referencefrom Reference , copyright , copyright (2018), Elsevier. (2018), Elsevier. On the other hand, soft templates mainly refer to the templates formed by organic surfactants, polymers,On the viruses, other hand, bacteria soft andtemplates bubbles mainly and sorefer forth. to the These templates materials formed can by self-assemble organic surfactants, into the orderedpolymers, structures viruses, bacteria under certain and bubbles conditions, and so such forth. as micellesThese materials or reverse can micelles, self-assemble emulsions into the or micro-emulsion,ordered structures vesicles under andcertain such. conditions, The target such substance as micelles or its or precursor reverse micelles, is typically emulsions nucleated or micro- on the surfaceemulsion, of thevesicles template and such. composed The targ of theseet substance ordered or structures. its precursor For is example, typically coral-likenucleatedCoSe on the could surface be preparedof the template via two-step composed solvothermal of these ordered reaction. structures Flower-like. For Co(OH) example,2 could coral-like be synthesized CoSe could using be prepared Pluronic P123via two-step (polyethylene-polypropylene solvothermal reaction. glycol) Flower-like as surfactants Co(OH)2 andcould then be followedsynthesized by anionusing exchangePluronic P123 . The(polyethylene-polypropylene prepared coral-like CoSe electrode glycol) as exhibit surfactant a lows overpotentialand then followed of 295 mVby anion to drive exchange a current . density The −2 −1 ofprepared 10 mA cmcoral-likewith CoSe a small electrode Tafel slope exhibit of 40 a mV low dec overpotential. Notably, of the 295 removal mV to of drive soft templatesa current isdensity easier thanof 10 thatmA ofcm the−2 with hard a templates; small Tafel therefore, slope of 40 the mV associated dec−1. Notably, template the damage removal to theof soft successively templates obtained is easier hierarchicalthan that of structure the hard can templates; then be minimized.therefore, the At theassociated same time, template the shell damage structure to the is oftensuccessively porous, whichobtained is beneﬁcialhierarchical to structure the exposure can then of active be minimize sites in thed. At inner the same hole. time, However, the shell as similar structure with is often hard templateporous, which methods, is beneficial the surface to the properties exposure of of the active template sites in and the the inner interaction hole. However, between as the similar template with andhard the template precursor methods, have a decisivethe surface effect properties on the formation of the template of hierarchical and the structures. interaction This between process the is inevitablytemplate and complicated, the precursor which have limits a thedecisive application effect on domains the formation of these softof hierarchical and hard template structures. methods. This processIn contrast,is inevitably the self-template complicated, method which islimits a scheme the application of synthesizing domains micro/nanoscale of these soft templatesand hard andtemplate then methods. transforming them into hierarchical structures. This way, the template not only acts as a physicalIn contrast, support the but self-template also directly method participates is a scheme in the formationof synthesizing of the micro/ shell layer.nanoscale Metal templates hydroxides, and metalthen transforming oxide and metal-organic them into hierarchical framework structures. (MOF) areThis all way, popular the template templates, not whichonly acts can as be a physical directly convertedsupport but into also a shelldirectly or asparticipates a precursor in tothe the form shellation [97 of–102 the]. shell For example,layer. Metal Lou’s hydroxides, group reported metal CoSeoxidex Sand2−[email protected](OH) metal-organic2 hierarchical framework nanotubes (MOF) as anare efﬁcient all popular OER catalyststemplates, [103 which]. Separate can selenylationbe directly andconverted sulfurization into a shell on the or Co(OH)as a precursor2 via the to anion-exchange the shell [97–102]. reactions For example, play an importantLou’s group role reported on the formationCoSexS2−[email protected](OH) of hierarchical2 hierarchical structures. nanotubes It is also as an noted efficient that OER MOF catalysts usually has. the Separate stable and selenylation uniform and sulfurization on the Co(OH)2 via the anion-exchange reactions play an important role on the formation of hierarchical structures. It is also noted that MOF usually has the stable and uniform shape, which the composition can be controlled rationally via selecting proper precursors and post-
Catalysts 2018, 8, 551 13 of 29 shape, which the composition can be controlled rationally via selecting proper precursors and post-treatment. [email protected] nanotubes derived from MOF were prepared successfully as an efﬁcient HER catalyst . The ﬁnal product possess the uniform morphology with an average size of 300 nm and as well with the surface surrounded by carbon nanotubes. This unique hierarchical structure can bring the excellent electrocatalytic performance, including a low onset potential of −1 40 mV and a small Tafel slope of 82 mV dec in 0.5 M H2SO4 solution. Yu’s group also reported the Ni-Co-MoS2 nanoboxes through the reaction between Prussian blue and ammonium thiomolybdate under solvothermal condition . Well-deﬁned cubic voids inside the nanoboxes are surrounded by ultrathin MoS2 nanosheets, which are clearly observed through TEM characterization. The same group as well constructed the NiS nanoframes using Prussian blue as the self-template scheme with the similar method . Furthermore, direct growth of active nanomaterials onto the three-dimensional conductive substrate is commonly adopted to prepare hierarchical structure. In this case, the clear solution contained with precursors of active material and the substrate are prepared. The hierarchical structure can be simply obtained via controlling the temperature and reaction time. Until now, nickel foam, iron foam, carbon paper and carbon ﬁber are all suitable candidates here. Evidently, huge amounts of work have already proved that the introduction of 3D substrate would substantially improve the corresponding electrocatalytic performance [105–107]. To be speciﬁc, our group prepared readily the ultrathin P-doped MoS2 nanosheets on carbon cloth . The synergistic effect between large surface area and modiﬁed active sites would make the P-doped (3.3 at.%) MoS2 nanosheets exhibiting the signiﬁcantly lower overpotentials of 133 and 189 mV to drive the current densities of 20 and 100 mA cm−2, respectively. Except these commercial substrates, metal oxide/hydroxide nanowire arrays on the 2D substrate can also a good choice here . Arrays of ZnSe/MoSe2 nanotubes on ﬂuorine doped tin oxide (FTO) glass substrates are synthesized and employed as an efﬁcient HER catalyst . The arrays of ZnO on FTO can also be functioned as 3D template for the subsequent modiﬁcation. All these can illustrate the versatility of all template-assisted methods for the formation of efﬁcient hierarchical electrocatalysts.
6.5. Self-Organized Nanostructures Different from the support/template method, the hierarchical structure synthesized via self-assembly schemes can be commonly controlled by a careful selection of solvents, reaction time, temperature, metal precursors and so on [95,111,112]. An example of a hierarchical structure formed by hydrothermal anion exchange method is shown in Figure5c. The formation of these hierarchical structures can be mainly divided into two stages: the nucleation stage and the growth stage. Uniquely, it is effective to control the thermodynamic and kinetic parameters to tune these two stages in order to reach the morphological control here . Particularly, the hierarchically nanostructured MoS2 nanosheets can be prepared as a HER catalyst in water-ethylene glycol mixture solution under solvothermal condition. As the ethylene glycol concentration increases, the morphologies evolve from nanoﬂowers and nanosheets to nanoﬂake aggregates. TEM characterization also conﬁrm that the nanosheets possess the rich in-plane edges reaching a low onset potential of 87 mV and a Tafel slope of 41 mV dec−1, indicating the usefulness of these self-organized nanostructures for high-performance hierarchical electrocatalysts.
7. Chemical Modiﬁcations for Improving Electrocatalytic Activity of TMCs After the initial research into binary TMCs showed promising results for electrocatalysts, a natural new direction of study was opened into ternary TMC systems featuring more complex blends. These can include binary TMCs that undergo doping or other post-synthesis treatments to introduce another component, or bottom-up synthesis methods that utilize varying precursor ratios to tune the composition. In this section, we will explore current results and trends regarding double anion, double cation and quaternary (i.e., double anion and double cation) TMC electrocatalysts. Catalysts 2018, 8, 551 14 of 29
7.1. Double Anion Ternary Transition Metal Chalcogenides as Electrocatalysts for Water Splitting Before they were widely studied as catalysts, double-anion TMCs such as mixed sulfur/selenium or partially oxidized sulﬁde had already seen research in other electronic or optical applications. However, their potential for HER catalysts was unique due to the possibility for these ternary blends to activate the basal plane in TMCs. Xie et al.  was among the ﬁrst to publish major research into double anion TMCs for HER. By controlling the synthesis temperature of a bottom-up synthesis reaction for MoS2 ﬂakes, the oxygen content was controlled, with lower temperature reaction conditions leading to increased oxygen content. The ﬂakes showing an increasing degree of disorder as the content increased, eventually becoming fully amorphous. The best performing sample (2.28 at.% O and 35–40% disordered) showed a Tafel slope of 55 mV/dec, a dramatic improvement over the pure MoS2 value of 81 mV/dec. This showed the potential of double anion TMCs and the importance of inducing disorder/defects in the basal plane. A similar strategy of defect creation and partial oxidation was used by Tao et al. , where the effects of Ar and O2 plasma on CVD MoS2 were studied. The formation of these defects as well as localized MoO3 was attributed to improve HER properties and the best sample (O2 plasma treated for 720 s) was shown to have a Tafel slope of 105 mV/dec compared to 160 mV/dec for the pristine MoS2. Although this type of defect creation and oxidation can successfully activate the basal planes of TMCs, another issue for TMCs is the charge transport from the electrocatalysts to the electrode, an issue that could be worsened by the amorphous or oxygen-rich regions of TMCs due to their lower electrical conductivity. To solve this issue, Zhang et al.  created amorphous MoSxCly supported by graphene. By using a low-temperature CVD process, the MoCl5 precursor was only partially sulfurized and did not crystallize. These composite samples showed outstanding HER properties, with the amorphous sample on vertical graphene requiring only −160 mV at 10 mA cm−2 and having a Tafel slope of only 46 mV/dec. Another popular strategy for double anion TMC catalysts is to substitute Se for S to induce a similar increase of active sites. Xu et al.  synthesized WS2(1−x)Se2x nanotubes by a transforming WO3 nanowires via a chemical vapor method, with the S/Se ratio controlled by varying the elemental precursors. Although the Tafel slope of the mixed-phase WS2(1−x)Se2x was not shown to be improved compared to pure WSe2 (105 mV/dec and 99 mV/dec, respectively), it was noted that the overpotential and current exchange density of WS2(1−x)Se2x was superior to pure WS2, WSe2, or WO3. Gong et al.  also created a mixed S/Se TMC through a bottom-up method using MoCl5 and varying the elemental S/Se added, as seen in Figure6b. Here, an even ratio of S and Se (MoSSe) was shown to be the most efﬁcient electrocatalyst. The work reported a Tafel slope of 48 mV/dec the overpotential at 10 mA cm2 of 164 mV, as well as 93% current density retention after 8000 cycles. The authors noted that previous theoretical work had suggested that sulﬁde Mo edges have a positive hydrogen adsorption energy (∆GH = 80 meV) , while selenide Mo edges have a negative adsorption energy (∆GH = −140 meV) . It was therefore suggested that the alloyed composition could reduce this value to near thermoneutral. Molybdenum sulfoselenide was also studied by Zhou et al.  by growth over a 3D porous NiSe2 foam (Figure6c). The underlying foam provided high surface area and a metallic electrical conduction pathway, while the MoS2(1−x)Se2x particles with vertically aligned layers provided the catalytically active sites. The Tafel slope and overpotential at 10 mA cm−2 were reported to be 42 mV/dec and 69 mV, respectively, both of which were much better than pure MoS2 over NiSe2 foam. Catalysts 2018, 8, 551 15 of 29 Catalysts 2018, 8, x FOR PEER REVIEW 15 of 29
Figure 6.Figure(a) Crystal 6. (a) Crystal structures structures of twoof two anion anion contain contain MoSSe with with changing changing the proton the proton energy energy and and band diagrams.band diagrams. Reprinted Reprinted with permission with permission from Referencefrom Reference [118 ],, copyright copyright (2017), (2017), American American Chemical Chemical Society. (b) Schematic illustration of MoSSe alloy formation and turnover frequency at η = Society. (b) Schematic illustration of MoSSe alloy formation and turnover frequency at η = 150 150 Mv for different compositions. Reprinted with permission from Reference , copyright (2015), Mv for differentAmerican Chemical compositions. Society. ( Reprintedc) The polarization with permissioncurves recorded from on MoS Reference2(1−x)Se2x/NiSe ,2 foam copyright hybrid, (2015), AmericanMoS Chemical2/NiSe2 foam Society. hybrid (c and) The pure polarization NiSe2 foam electrodes curves recorded compared on with MoS a Pt2(1 wire−x)Se .2x/NiSe (d) By2 takingfoam hybrid, MoS2/NiSeadvantage2 foam of hybrid the electrostatic and pure attraction NiSe2 foambetwee electrodesn the two oppositely compared charged with nanosheets, a Pt wire [ [email protected]]. (dr)GO By taking advantagecomposite of the electrostaticmaterials are obtained attraction exhi betweenbiting superior the two electrocatalytic oppositely activity charged and nanosheets, stability for the [email protected] HER rGO −2 compositeallowing materials a current are density obtained of 5 exhibiting mA cm at superior a low overpotential electrocatalytic of only activity135 mV. andReprinted stability with for the permission from Reference , copyright (2016), Elsevier. HER allowing a current density of 5 mA cm−2 at a low overpotential of only 135 mV. Reprinted with permissionAlthough from ReferenceS and Se are [119 far], more copyright widely (2016), researched, Elsevier. Te is another chalcogen that can be utilized to create efficient HER catalysts. Kosmala et al.  synthesized MoSe2−xTex films through molecular Althoughbeam epitaxy S and and Se reported are far more a Tafel widely slope and researched, overpotential Te isat another10 mA cm chalcogen−2 of 62 mV/dec that and can 410 be mV, utilized to create efﬁcientrespectively. HER The catalysts. authors Kosmala showed etthat al. the [120 syst] synthesizedem contains MoSemany2 −metallicxTex ﬁlms twin through boundaries, molecular beam epitaxythermodynamically and reported stable a Tafeldefects slope whichand can overpotentialincrease catalytic at activity. 10 mA Interestingly, cm−2 of 62 the mV/dec ideal and 410 mV,composition respectively. was The found authors to be Te-rich showed (MoSe that0.12Te the1.79) systemand it was contains also noted many that the metallic pristinetwin MoTe boundaries,2 was far more catalytically active that the pristine MoSe2 prepared under the same conditions. This is a thermodynamically stable defects which can increase catalytic activity. Interestingly, the ideal result that contradicts previous computational  and experimental  research that had compositionsuggested was tellurides found to would be Te-rich not be (MoSe as intrinsically0.12Te1.79) catalytically and it was active also noted as sulfides that theor selenides. pristine MoTe2 was far moreTherefore, catalytically research into active telluride-based that the pristine TMC cataly MoSests may2 prepared be an avenue under worth the samefurther conditions. exploration. This is a result that contradicts previous computational  and experimental  research that had suggested tellurides would not be as intrinsically catalytically active as sulﬁdes or selenides. Therefore, research into telluride-based TMC catalysts may be an avenue worth further exploration. Other anions explored for substitution into TMCs include nitrogen, which was studied by Sun et al.  to create N-doped WS2 nanosheets through a one-step sol-gel process using WCl6 and thiourea followed by post-annealing in H2. The work demonstrated a Tafel slope of 70 mV/dec and no CatalystsCatalysts2018, 8 2018, 551, 8, x FOR PEER REVIEW 16 of 29 16 of 29
Other anions explored for substitution into TMCs include nitrogen, which was studied by Sun signiﬁcantet al. loss ofto currentcreate N-doped density WS over2 nanosheets 10 h at 200 through mV. Like a one-step other doublesol-gel process anion TMCs,using WCl the6 resultand was attributedthiourea to increased followed by active post-annealing sites due toin H defect2. The formation.work demonstrated a Tafel slope of 70 mV/dec and Phosphorusno significant substitution loss of current was density recently over 10 studied h at 200 by mV. Liu Like et al.other [124 double] using anion a bottom-up TMCs, the result method to was attributed to increased active sites due to defect formation. create P-doped MoS2 nanosheets. A doping level of up to 5 at.% was achieved and this sample showed Phosphorus substitution was recently studied by Liu et al.  using a bottom-up method to outstanding catalytic properties, including a Tafel slope of 34 mV/dec, which is extremely close to the create P-doped MoS2 nanosheets. A doping level of up to 5 at.% was achieved and this sample showed referenceoutstanding Pt/C benchmark catalytic properties, catalyst including (30 mV/dec). a Tafel sl Interestingly,ope of 34 mV/dec, the which performance is extremely enhancement close to the was attributedreference to not Pt/C only benchmark the increased catalyst active (30 mV/dec). sites but Interestingly, also an improvement the performance in the enhancement electrical conductivity was due toattributed increased to chargenot only carriers. the increased In addition, active sites the but expanded also an improvement interlayer distancein the electrical of the conductivity P-doped sample (0.91 nm)due to compared increased tocharge the referencecarriers. In MoSaddition,2 (0.65 the nm) expanded was asserted interlayer to distance lower of the the∆ GP-dopedH value. sample Due(0.91 to nm) the compared wide availability to the reference of both MoS dopant2 (0.65 nm) anions was asserted and synthesis to lower the methods ΔGH value. available to create double anionDue TMCs,to the wide it is likelyavailability that of research both dopant in this an directionions and synthesis will continue methods to progress.available to It create is possible double anion TMCs, it is likely that research in this direction will continue to progress. It is possible that future works will combine double anion active materials with the conductive supports previously that future works will combine double anion active materials with the conductive supports discussed,previously such discussed, as MoSSe/rGO such as MoSSe/rGO catalysts shown catalysts in shown Figure in6d Figure [ 118 ].6d It. is worth It is worth noting noting that that all work reportedall work to date reported has used to date methods has used that methods cannot that produce cannot any produce sort of any regular sort of ordering regular ordering or arrangement or of thearrangement substituting of atoms. the substituting It is possible atoms. that It is possibl periodice that or periodic ordered or double ordered anion double structures, anion structures, such as the “Janus”such TMCs as the suggested “Janus” TMCs by recent suggested theoretical by recent works theoretical [62,116 works,125] would[62,116,125] yield would unique yield electrocatalytic unique properties.electrocatalytic In these properties. structures, In thes onee structures, side of the one transition side of the metaltransition (W metal or Mo) (W or is Mo) sulfurized is sulfurized while the other iswhile selenide the other (illustrated is selenide in (illustrated Figure7a). in However, Figure 7a). the However, only reported the only synthesis reported synthesis method [method65] for these  for these structures is a complex and multi-step process, which may limit research into their structures is a complex and multi-step process, which may limit research into their potential for HER potential for HER catalysts. We also predict that strategies utilizing naturally high surface area catalysts.starting We alsomaterials predict such that as Ni strategies foam (shown utilizing in Figu naturallyre 7b,c) highwill receive surface growing area starting interest materials in the near such as Ni foamfuture. (shown in Figure7b,c) will receive growing interest in the near future.
Figure 7. (a) Schematic for WSSe with ∆ GH “volcano” plot, the illustration shows that strain free Janus TMDs possess better HER activities. Reprinted with permission from , copyright (2018), American Chemical Society. (b) TEM of WS2(1−x)Se2x particles with a 3D porous metallic NiSe2 foam and corresponding polarization curves recorded on WS2(1−x)Se2x/NiSe2 foam. (c) TEM of WS2(1−x)Se2x nanotubes and corresponding polarization curves recorded on WS2(1−x)Se2x in comparison with WS2. Reprinted with permission from Reference , copyright (2014), American Chemical Society. Catalysts 2018, 8, x FOR PEER REVIEW 17 of 29
Figure 7. (a) Schematic for WSSe with Δ GH “volcano” plot, the illustration shows that strain free Janus TMDs possess better HER activities. Reprinted with permission from , copyright (2018),
American Chemical Society. (b) TEM of WS2(1−x)Se2x particles with a 3D porous metallic NiSe2 foam
Catalysts 2018and ,corresponding8, 551 polarization curves recorded on WS2(1−x)Se2x/NiSe2 foam. (c) TEM of WS2(1−x)Se2x 17 of 29 nanotubes and corresponding polarization curves recorded on WS2(1−x)Se2x in comparison with WS2. Reprinted with permission from Reference , copyright (2014), American Chemical Society. 7.2. Double Cation Ternary Transition Metal Chalcogenides as Electrocatalysts for Water Splitting 7.2. Double Cation Ternary Transition Metal Chalcogenides as Electrocatalysts for Water Splitting Like double anion TMC catalysts, double cation catalysts have been extensively studied as HER catalysts.Like In double many anion ways, TMC the corecatalysts, goals double are similar cation incatalysts both cases, have been namely, extensively to disrupt studied the as normally HER catalysts. In many ways, the core goals are similar in both cases, namely, to disrupt the normally inactive basal plane and create addition active sites through defect or strain formation. However, inactive basal plane and create addition active sites through defect or strain formation. However, because the transition metal atoms are generally not adsorption sites for layered TMC materials, because the transition metal atoms are generally not adsorption sites for layered TMC materials, many works have suggested that the beneﬁt of double cation TMCs may be more attributable to many works have suggested that the benefit of double cation TMCs may be more attributable to electron density and local ﬁeld effects, as illustrated in Figure8a . electron density and local field effects, as illustrated in Figure 8a . Li et al.  synthesized Mo − WxS2 using a hydrothermal method with Na2MoO4·H2O Li et al.  synthesized Mo(1(1−x)x)WxS2 using a hydrothermal method with Na2MoO4∙H2O and and Na WO ·H O in varying ratios and analyzed the effect of cation ratio on HER performance. Na2WO2 4∙H42O in2 varying ratios and analyzed the effect of cation ratio on HER performance. The TheMo Mo0.850.85W0.15WS0.152 compositionS2 composition showed showed the best the electrocatalytic best electrocatalytic properties, properties, including including a Tafel slope a Tafel of slope 89 ofmV/dec 89 mV/dec and andstability stability demonstrated demonstrated for 1000 for cycles. 1000 cycles.Using DFT Using calculations, DFT calculations, it was shown it was that shown the thatband the gap band of gapMoWS of2 MoWS (0.88 eV)2 (0.88 waseV) smaller was than smaller that thanof MoS that2 (1.14 of MoS eV)2 and(1.14 that eV) W and atoms that create W atoms an create“electron-rich” an “electron-rich” configuration conﬁguration through through directional directional transfer. transfer. It was It wasasserted asserted that that this this electronic electronic modiﬁcationmodification improves improves the the conductivity conductivity and and therefore therefore decreasesdecreases the charge transfer transfer resistance. resistance.
Figure 8. (a) Unfolded energy band of two cations contains ternary Mo1−xWxS2. Reprinted with permissionFigure 8. from(a) Unfolded Reference energy , copyrightband of two (2017), cations Scientiﬁc contains Reports. ternary (bMo) Schematic1−xWxS2. Reprinted illustration with for permission from Reference , copyright (2017), Scientific Reports. (b) Schematic illustration for the the formation of Mo1−xWxS2 and Mo1−xWxS3 and corresponding polarization curves recorded on formation of Mo1−xWxS2 and Mo1−xWxS3 and corresponding polarization curves recorded on Mo1−xWxS2 Mo1−xWxS2 and Mo1−xWxS3. Reprinted with permission from Reference , copyright (2017), and Mo1−xWxS3. Reprinted with permission from Reference , copyright (2017), American American Chemical Society. Chemical Society.
Tan and Pumera  synthesized composition-graded, sulfur-deﬁcient MoWSx. The material was initially synthesized through electrodeposition using (NH4)2MoS4 and (NH4)2WS4 dissolved in 0.1 M KCl solution (Figure8b). Because these were synthesized using bipolar deposition, two distinct compositions were designated based on whether the deposition was cathodic (creating MoxW(1−x)S2) −2 or anodic (creating MoxW(1−x)S2). The Tafel slope and overpotential at 10 mA cm for the samples were 45.7 mV/dec and 315 mV for the cathodic sample and 50.5 mV/dec and 278 mV for the anodic sample. The even Mo/W ratio and high exposed surface are of the small particles were cited as the primary reasons for the increased performance compared to pure MoS2 or WS2. Catalysts 2018, 8, 551 18 of 29
Several other works have reported similar Mo/W mixtures for HER catalysts, including Li et al.  reporting MoWS on carbon cloth and Gan et al.  demonstrating MoXWyS2 supported by pyrolytic carbon. These works consistently report that the mixed systems outperform the single-cation TMCs but the ideal Mo/W ratio for HER activity is different for each study. This indicates that differences in processing conditions or supporting structures may greatly affect the ideal composition. Many other metals have been studied for TMC catalysts in the form of cation dopants. Shi et al.  studied MoS2 doped with a variety of metals: Co, Cu, Fe, Ni and Zn. Zn was shown to be the best dopant, with a Tafel slope of 51 mV/dec representing a dramatic improvement over the pristine MoS2 value (101 mV/dec). The improvement was attributed to both energy level modiﬁcation and morphological effects induced by Zn doping. However, not all dopant cations have shown improved catalytic performance. Chua et al.  reported that both niobium and tantalum doing in MoS2 and WS2 failed to improve the HER −2 performance and the undoped MoS2 showed the best overpotential at 10 mA cm of any of the tested samples. This result was particularly notable because the authors conﬁrmed the increased presence of the 1T metallic phase after doping, which had been shown to be beneﬁcial in other HER studies [131,132]. In addition, Tsai et al.  had computationally predicted that many types of cation dopants, including Ta and Nb, would bring the ∆GH value closer to thermoneutral and beneﬁt HER properties. Although not technically ‘double’ cation catalysts, Askari et al.  synthesized two mixed cation systems—MoWCoS and MoWCuS—by a hydrothermal method using sodium molybdate, sodium tungstate and either cobalt chloride or copper chloride as precursors. When hybridized with reduced graphene oxide, the MoWCoS showed particularly strong HER properties, with the Tafel slope and overpotential reported to be 38 mV/dec. It was asserted that the CoS phases present within the material create new interfaces and introduce additional defects, greatly increasing the catalytic activity. A more unusual TMC system was studied by Zhan et al. : Ag2WS4 prepared through a ◦ low-temperature (60 C) ion-exchange reaction using (NH4)WS4 and AgNO3 precursors. The sample showed a Tafel slope of 62 mV/dec and was stable for 24 h. Edge-sharing of AgS4 and WS4 tetrahedra was asserted to create numerous active sites. We do note that the use of silver undermines the typical goal of “noble-metal free catalysts” that is often stated in HER research. However, the price of silver is still far less than that of typical benchmark noble metal for electrocatalytic reactions (i.e., Pt and Ru). Zhou et al.  created another TMC based on a rarely-studied metal by coating MoSx on NbS2 nanoﬂakes. The initial NbS2 over glassy carbon (GC) was synthesized by CVD followed drop casting over glassy carbon (GC) and coating with ammonium thiomolybdate to create [email protected]/CG electrocatalysts. The sample showed solid HER performance, with a Tafel slope of 43.2 mV/dec and an overpotential of −164 mV at −10 mA cm−2. The authors also noted that the performance at high current densities was particularly strong; the overpotential at −200 mA cm−2 (−233 mV) was claimed to be even lower than that of the commercial Pt/C catalyst (−274 mV). It was shown that the interface region creates numerous S vacancies in MoSx, which lowers the ∆GH value. In addition to W and Mo-based TMCs, many other metals have been studied for use in HER catalysts. Amin et al. synthesized CoNi2Se4 via electrodeposition for overall water splitting (i.e., OER and HER). The vacancy-ordered spinel structure was shown to be a highly efﬁcient OER catalyst but the HER properties were not as impressive: the overpotential was reported as 220 mV at 10 mA cm−2. Like mixed anion TMC HER catalysts, it is likely that this direction will also continue to see a wide range of research interest. However, the exact role of the mixed cation seems to be slightly less clear than that of mixed anion systems, with many different suggested mechanisms claimed to be responsible for performance enhancements (electron density modulation, 2H/1T phase transformation, morphological effects, etc.). For this reason, more fundamental studies and detailed investigations into the roles of speciﬁc cation dopants would undoubtedly be beneﬁcial for future HER research. Catalysts 2018, 8, x FOR PEER REVIEW 19 of 29 and HER). The vacancy-ordered spinel structure was shown to be a highly efficient OER catalyst but the HER properties were not as impressive: the overpotential was reported as 220 mV at 10 mA cm−2. Like mixed anion TMC HER catalysts, it is likely that this direction will also continue to see a wide range of research interest. However, the exact role of the mixed cation seems to be slightly less clear than that of mixed anion systems, with many different suggested mechanisms claimed to be responsible for performance enhancements (electron density modulation, 2H/1T phase transformation, morphological effects, etc.). For this reason, more fundamental studies and detailed investigations into the roles of specific cation dopants would undoubtedly be beneficial for future HERCatalysts research.2018, 8, 551 19 of 29
7.3. Quaternary Transition Metal Chalcogenides as Electrocatalysts for Water Splitting 7.3. Quaternary Transition Metal Chalcogenides as Electrocatalysts for Water Splitting Because both mixed anion and mixed cation systems have shown better HER properties than their Becausebinary reference both mixed materials, anion andcombining mixed cationthese two systems approaches have shown to create better quaternary HER properties systems thanwas atheir natural binary next reference step in materials, electrocatalyst combining research. these Compared two approaches to the to double create quaternaryanion and systemsdouble cation was a works,natural this next approach step in electrocatalyst has not yet seen research. as much Compared published to research the double but it anion is likely and to double grow in cation popularity works, asthis the approach standards has for not electrocatalytic yet seen as much performance published research increase but and it isresearchers likely to grow looks in for popularity new ways as theto innovate.standards for electrocatalytic performance increase and researchers looks for new ways to innovate. Tiwari et al. [64] synthesized a quaternary TMC through a bottom-up direct reaction using [Cu(MeCN)](BF44), (NH 4))22[MoS[MoS44] ]and and diphenyl diphenyl diselenide diselenide (DPDS) (DPDS) (Figure (Figure 99a).a). By adjusting thethe DPDSDPDS concentration, the ratioratio ofof SS toto SeSe couldcould be be tuned, tuned, creating creating Cu Cu2Mo(S2Mo(SySeySe1−1−y))44.. The The sample sample with with ~3 ~3 at.% at.% Se doping showed showed the the best best HER HER properties: properties: 52 52 mV/dec mV/dec Tafel Tafel slope slope and and −170−170 mV mV overpotential overpotential at 10 at −2 10mA mA cm cm−2. DFT. DFT calculations calculations suggested suggested that that similar similar to toSe Se substitution substitution in in previously previously studied studied ternary ternary TMCs, Se substitution increases the numbernumber of active sites and reduces thethe ∆ΔGGHH value.
Figure 9. ((a)) Schematic illustrationillustration ofof HERHER activityactivity on on single single layer layer Cu Cu2Mo(S2Mo(S1−1−yySey))44 andand corresponding corresponding polarization curves andand TafelTafel plotsplots forfor single single and and multi-layer multi-layer Cu Cu2Mo(S2Mo(S1−1y−SeySeyy))44. Reprinted Reprinted with permission fromfrom ReferenceReference [64,], copyright copyright (2016), (2016), Elsevier. Elsevier. (b ()b Schematic) Schematic illustration illustration of of HER HER activity activity on onCu 2W(SCu2W(S1−ySe1−yySe)4yand)4 and corresponding corresponding polarization polarization curves curves and Tafel and plots Tafel for Cuplots2W(S for1−y SeCuy)24W(S. Reprinted1−ySey)4. Reprintedwith permission with permission from Reference from [Reference137], copyright , (2018),copyright Royal (2018), Society Royal of Chemistry.Society of Chemistry.
Later, Kim et al. [138] usedused aa similarsimilar methodmethod toto synthesizesynthesize CuCu22MoS4 and decorated the surface with MoSe MoSe22 nanodots.nanodots. The The nanodot nanodot size size and and concentratio concentrationn was was optimized optimized and andthe authors the authors found found that thethat smallest the smallest diameter diameter nanodots nanodots (30 nm) (30 nm) were were most most effective effective at enhancing at enhancing HER HER performance performance due due to theirto their higher higher surface surface area. area. The The optimized optimized sample sample showed showed a aTafel Tafel slope slope of of 74.7 mV/decmV/dec and and an overpotential of 166 mV at mA cm−2, with the mechanism of enhancement claimed to be the additional active sites created by the MoSe2 nanodots. Recently, Tiwari et al.  also used the previously reported selenium doping technique  in the Cu2WS4 system to synthesize Cu2W(SySe1−y) (Figure9b). The Tafel slope and overpotential −2 at 10 mA cm for the best sample (Cu2WS1.3Se2.7) were reported to be 46 mV/dec and 320 mV, respectively. It was concluded through XRD and Raman analysis that the Se substation created chemical strain in the lattice, lowering the ∆GH value and creating a greater number of active sites. Catalysts 2018, 8, x FOR PEER REVIEW 20 of 29
overpotential of 166 mV at mA cm−2, with the mechanism of enhancement claimed to be the additional active sites created by the MoSe2 nanodots. Recently, Tiwari et al.  also used the previously reported selenium doping technique  in the Cu2WS4 system to synthesize Cu2W(SySe1−y) (Figure 9b). The Tafel slope and overpotential at 10 Catalysts 2018, 8, 551 20 of 29 mA cm−2 for the best sample (Cu2WS1.3Se2.7) were reported to be 46 mV/dec and 320 mV, respectively. It was concluded through XRD and Raman analysis that the Se substation created chemical strain in the lattice,A thorough lowering study the of Δ theGH compositionvalue and creating compositional a greater effects number using of Mo,active W, sites. S and Se was performed by GongA thorough et al. [139 study], where of the 25 differentcomposition compositions compositional were synthesizedeffects using through Mo, W, a solution-phaseS and Se was method.performed The by work Gong identiﬁed et al. , WS where2, Mo 0.6725 differentW0.33S2, Mocompositions0.5W0.5SSe andwere Mo synthesized0.33W0.67S1.33 throughSe0.67 asa solution- the best performingphase method. compositions The work identified and noted WS that2, Mo in general0.67W0.33S the2, Mo ternary0.5W0.5 orSSe quaternary and Mo0.33W catalysts0.67S1.33Se outperformed0.67 as the best theirperforming binary compositions counterparts. and A summary noted that of in the general electrocatalytic the ternary performance or quaternary of catalysts all 25 compositions outperformed is showntheir binary in Figure counterparts. 10. A summary of the electrocatalytic performance of all 25 compositions is shown in Figure 10.
FigureFigure 10.10. Summarizing the onset overpotential, Tafel slope and TOF @ η == 160 mV ofof differentdifferent compositions.compositions. The The red red color labels compositionscompositions withwith TOFTOF >> 0.10.1 ss−−1;; the magentamagenta colorcolor labelslabels compositionscompositions withwith 0.060.06 << TOFTOF < < 0.10.1 s s−−1;; the blue colorcolor labelslabels compositionscompositions withwith 0.04 0.04 < < TOF TOF < < 0.06 0.06 s −s−11. AdaptedAdapted withwith permissionpermission fromfrom ReferenceReference [,139], copyrightcopyright (2016),(2016), Wiley-VCH.Wiley-VCH.
AnotherAnother quaternaryquaternary systemsystem waswas reportedreported byby WangWang etet al.al. [140] byby usingusing a carbothermal ammonia reductionreduction strategystrategy overover nickelnickel foamfoam toto synthesizesynthesize MoNiNC.MoNiNC. TheThe optimizedoptimized structuresstructures delivereddelivered aa −2 TafelTafel slopeslope ofof 6565 mV/decmV/dec andand overpotentialoverpotential atat 1010 mAmA cmcm−2 ofof 110 mV. AlthoughAlthough notnot technicallytechnically aa chalcogenide,chalcogenide, work is is notable notable because because DFT DFT calculations calculations revealed revealed that that both both the thedouble double metal metal (Mo (Moand andNi) as Ni) well as wellas the as double the double anion anion(N and (N C) and weaken C) weaken the bond the strength bond strength between between the active the site active and sitethe andadsorbed the adsorbed reactive reactive intermediate, intermediate, resulting resulting in improved in improved HER HER properties. properties. This This proves proves that that thethe synergisticsynergistic effectseffects of quaternaryof quaternary TMCs TMCs is a research is a research avenue worthavenue further worth development further development and exploration. and A summary of the performance data of binary, ternary and quaternary catalysts can be found in Table1.
Catalysts 2018, 8, 551 21 of 29
−2 Table 1. Performance data of various catalysts, showing the overpotential at 10 mA cm (η10) and Tafel slopes.
Type Composition Structure η10 (mV) Tafel (mV/dec) Ref. WSe2 Nanotubes 365 99 
MoS2 [email protected] 130 41  Binary MoS2 167 70 Hierarchical nanosheets  WS2 157 60
MoSe2 3D hierarchical 317 47  MoSxOy Nanosheets 120 55 
MoSxCly [email protected] 160 46  MoSxSey Nanoﬂakes 164 48  Ternary (double anion) MoSexTey Thin ﬁlms 410 62 
N-doped WS2 Nanosheets 127 70 
P-doped MoS2 Nanosheets 43 34  MoWSx Thin ﬁlm 315 46  MoWS [email protected] cloth 198 54 
MoxW1−xS2 Nanoﬂ[email protected] 137 53 
Zn-doped MoS2 Roselike nanosheets 110 51  Ternary (double cation) Ta-doped MoS 660 265 2 Micro particles  Nb-doped MoS2 680 190 MoWCoS [email protected] 282 41 
Ag2WS4 Micro-cubes 320 62 
[email protected] Nanoﬂakes 164 43 
Cu2Mo(SySe1−y)4 Nanosheets 170 52  MoSe @Cu MoS [email protected] 176 75  Quaternary 2 2 4 Cu2W(SySe1−y) Nanoparticles 320 46  MoNiNC [email protected] foam 110 65 
8. Conclusions We have summarized the recent progress in the development of ternary and quaternary TMCs as electrocatalysts for the water splitting especially for HER. To date, different types of TMCs electrodes consisting of various structures and chemical compositions (including nanoparticles, nanosheets, ﬁlms and composites) have exhibited excellent HER efﬁciencies. It is revealed that to improve the catalytic activity of TMCs, two main strategies are being pursued: (i) structure engineering of TMCs to expose additional active sites or provide conductive pathways to fully utilize the materials’ catalytic potential (extrinsic) and (ii) chemical modiﬁcation through heteroatom substitution to enhance hydrogen adsorption by decreasing the ∆GH values (intrinsic). However, many challenges remain associated with the use of TMCs as electrocatalysts. The electrocatalytic activities are affected by the morphology, structure and density of active sites, therefore, close attention should be paid to the speciﬁc surface area and chemical composition of the designed TMCs electrocatalysts. In this regards, TMCs consisting of small nanoparticles or containing heterostructures with conductive materials have shown great advantages due to their large number of active sites and high conductivity but these kind of materials are easy to aggregate and show poor stability. The strategy to form ternary or quaternary TMCs electrodes may be a feasible way to solve stability problem. In the case of ternary and quaternary with rich active sites, shows great promises for scalable application but further utilization of inactive basal planes remains to be undertaken. As for the hierarchical structures of TMCs on conductive template or self-organized nanostructures can be effective way to further utilizations of active sites for efﬁcient electrocatalytic activity. For this method, the ease of preparation, cost-effectiveness, repeatability and stability are all important factors which would strongly affect the practical applications of all these catalysts. Catalysts 2018, 8, 551 22 of 29
In addition, the improvement of the inherent activity of TMCs electrocatalysts is important for efﬁcient electrocatalytic activity for water splitting. Potential strategies to improve inherent activity include elemental substitution in host TMCs materials. Although this heteroatom substitution method has not been realized for active edge sites of TMCs, chalcogen-atom substitution to form chemical strain for activation of basal planes is a good example showing how such an effect could be realized. However, substitution near the active edge sites of TMCs still need further investigation to provide clear insight for the efﬁcient electrocatalytic activity. Further study could be focus on biomimetic and molecular catalysts using discrete molecular units as catalysts for efﬁcient electrocatalytic activity. Stabilization of molecular catalysts with suitable substrates, such as metal organic framework (MOF) and ﬁnding bimetallic organometallic complexes with terminal chalcogen ligands could provide another insight for non-noble metal electrocatalysts. Owing to the demand for renewable energy, the ﬁeld of the electrochemical water splitting using TMCs as electrocatalyst has been experiencing a renaissance in recent years. Despite encouraging results in research laboratory, few results have demonstrated the use of TMCs electrocatalysts in large-scale applications. Thus, a great deal of effort is still needed for further expanding the search for high-performance electrocatalysts and exploring the practical use of the efﬁcient advanced electrocatalysts.
Funding: This work was supported by the National Research Foundation of Korea (NRF) under grant no. NRF-2017R1D1A1B03032791, National Research Foundation of Korea (NRF) under grant no. NRF-2016M3A7B4900119 and, Nano-Material Technology Development Program through the National Research Foundation of Korea (NRF) funded by the Ministry of Science, ICT and Future Planning grant no. NRF-2017M3A7B4041987. Conﬂicts of Interest: The authors declare no conﬂict of interest.
1. Walter, M.G.; Warren, E.L.; McKone, J.R.; Boettcher, S.W.; Mi, Q.; Santori, E.A.; Lewis, N.S. Solar Water Splitting Cells. Chem. Rev. 2010, 110, 6446–6473. [CrossRef][PubMed] 2. Balat, M.; Balat, H. Biogas as a Renewable Energy Source—A Review. Energy Sources Part A Recover. Util. Environ. Effects 2009, 31, 1280–1293. [CrossRef] 3. Shi, L.; Zhao, T. Recent advances in inorganic 2D materials and their applications in lithium and sodium batteries. J. Mater. Chem. A 2017, 5, 3735–3758. [CrossRef] 4. Das, S.; Pandey, D.; Thomas, J.; Roy, T. The Role of Graphene and Other 2D Materials in Solar Photovoltaics. Adv. Mater. 2018, 1802722. [CrossRef][PubMed] 5. Withers, F.; Del Pozo-Zamudio, O.; Mishchenko, A.; Rooney, A.P.; Gholinia, A.; Watanabe, K.; Taniguchi, T.; Haigh, S.J.; Geim, A.K.; Tartakovskii, A.I.; et al. Light-emitting diodes by band-structure engineering in van der Waals heterostructures. Nat. Mater. 2015, 14, 301. [CrossRef][PubMed] 6. Azam, A.; Kim, J.; Park, J.; Novak, T.G.; Tiwari, A.P.; Song, S.H.; Kim, B.; Jeon, S. Two-Dimensional
WO3 Nanosheets Chemically Converted from Layered WS2 for High-Performance Electrochromic Devices. Nano Lett. 2018, 18, 5646–5651. [CrossRef][PubMed] 7. Novak, T.G.; Shin, H.; Kim, J.; Kim, K.; Azam, A.; Nguyen, C.V.; Park, S.H.; Song, J.Y.; Jeon, S. Low-Cost Black Phosphorus Nanoﬁllers for Improved Thermoelectric Performance in PEDOT:PSS Composite Films. ACS Appl. Mater. Interfaces 2018, 10, 17957–17962. [CrossRef][PubMed] 8. Dong, Y.; Mallineni, S.S.K.; Maleski, K.; Behlow, H.; Mochalin, V.N.; Rao, A.M.; Gogotsi, Y.; Podila, R. Metallic MXenes: A new family of materials for ﬂexible triboelectric nanogenerators. Nano Energy 2018, 44, 103–110. [CrossRef] 9. Turner, J.A. Sustainable Hydrogen Production. Science 2004, 305, 972–974. [CrossRef][PubMed] 10. Dresselhaus, M.S.; Thomas, I.L. Alternative energy technologies. Nature 2001, 414, 332. [CrossRef][PubMed] 11. Rostrup-Nielsen, J.R. Fuels and Energy for the Future: The Role of Catalysis. Catal. Rev. 2004, 46, 247–270. [CrossRef] 12. Bockris, J.O.M. The origin of ideas on a Hydrogen Economy and its solution to the decay of the environment. Int. J. Hydrogen Energy 2002, 27, 731–740. [CrossRef] Catalysts 2018, 8, 551 23 of 29
13. Lasia, A. Hydrogen evolution reaction. In Handbook of Fuel Cells; John Wiley & Sons, Ltd.: Hoboken, NJ, USA, 2010. [CrossRef]
14. Phuruangrat, A.; Ham, D.J.; Thongtem, S.; Lee, J.S. Electrochemical hydrogen evolution over MoO3 nanowires produced by microwave-assisted hydrothermal reaction. Electrochem. Commun. 2009, 11, 1740–1743. [CrossRef] 15. Kotrel, S.; Bräuninger, S. Industrial Electrocatalysis. In Handbook of Heterogeneous Catalysis; Wiley-VCH Verlag GmbH & Co. KGaA: Weinheim, Germany, 2008. 16. Nørskov, J.K.; Bligaard, T.; Logadottir, A.; Kitchin, J.R.; Chen, J.G.; Pandelov, S.; Stimming, U. Trends in the Exchange Current for Hydrogen Evolution. J. Electrochem. Soc. 2005, 152, J23–J26. [CrossRef] 17. Chen, J.; Lim, B.; Lee, E.P.; Xia, Y. Shape-controlled synthesis of platinum nanocrystals for catalytic and electrocatalytic applications. Nano Today 2009, 4, 81–95. [CrossRef] 18. Greeley, J.; Jaramillo, T.F.; Bonde, J.; Chorkendorff, I.; Nørskov, J.K. Computational high-throughput screening of electrocatalytic materials for hydrogen evolution. Nat. Mater. 2006, 5, 909. [CrossRef][PubMed] 19. Morales-Guio, C.G.; Stern, L.-A.; Hu, X. Nanostructured hydrotreating catalysts for electrochemical hydrogen evolution. Chem. Soc. Rev. 2014, 43, 6555–6569. [CrossRef][PubMed] 20. Faber, M.S.; Jin, S. Earth-abundant inorganic electrocatalysts and their nanostructures for energy conversion applications. Energy Environ. Sci. 2014, 7, 3519–3542. [CrossRef] 21. Gao, M.-R.; Xu, Y.-F.; Jiang, J.; Yu, S.-H. Nanostructured metal chalcogenides: Synthesis, modiﬁcation, and applications in energy conversion and storage devices. Chem. Soc. Rev. 2013, 42, 2986–3017. [CrossRef] [PubMed] 22. Chhowalla, M.; Shin, H.S.; Eda, G.; Li, L.-J.; Loh, K.P.; Zhang, H. The chemistry of two-dimensional layered transition metal dichalcogenide nanosheets. Nat. Chem. 2013, 5, 263. [CrossRef][PubMed] 23. Voiry, D.; Yang, J.; Chhowalla, M. Recent Strategies for Improving the Catalytic Activity of 2D TMD Nanosheets Toward the Hydrogen Evolution Reaction. Adv. Mater. 2016, 28, 6197–6206. [CrossRef] [PubMed] 24. Bard, A.J.; Faulkner, L.R. Electrochemical Methods: Fundamentals and Applications; John Wiley & Sons: Hoboken, NJ, USA, 2007. 25. Godula-Jopek, A. Hydrogen Production by Electrolysis; Wiley-VCH: Weinheim, Germany, 2015. 26. Bockris, J.O.M.; Potter, E.C. The Mechanism of the Cathodic Hydrogen Evolution Reaction. J. Electrochem. Soc. 1952, 99, 169–186. [CrossRef] 27. Trasatti, S. Work function, electronegativity, and electrochemical behaviour of metals: III. Electrolytic hydrogen evolution in acid solutions. J. Electroanal. Chem. Interfacial Electrochem. 1972, 39, 163–184. [CrossRef]
28. Tributsch, H.; Bennett, J.C. Electrochemistry and photochemistry of MoS2 layer crystals. I. J. Electroanal. Chem. Interfacial Electrochem. 1977, 81, 97–111. [CrossRef] 29. Gileadi, E. Physical Electrochemistry: Fundamentals, Techniques and Applications; John Wiley & Sons: Hoboken, NJ, USA, 2011. 30. Carmo, M.; Fritz, D.L.; Mergel, J.; Stolten, D. A comprehensive review on PEM water electrolysis. Int. J. Hydrogen Energy 2013, 38, 4901–4934. [CrossRef] 31. Giovanni, C.D.; Reyes-Carmona, Á.; Coursier, A.; Nowak, S.; Grenèche, J.M.; Lecoq, H.; Mouton, L.; Rozière, J.; Jones, D.; Peron, J.; et al. Low-Cost Nanostructured Iron Sulﬁde Electrocatalysts for PEM Water Electrolysis. ACS Catal. 2016, 6, 2626–2631. [CrossRef] 32. Seh, Z.W.; Kibsgaard, J.; Dickens, C.F.; Chorkendorff, I.; Nørskov, J.K.; Jaramillo, T.F. Combining theory and experiment in electrocatalysis: Insights into materials design. Science 2017, 355, eaad4998. [CrossRef] [PubMed] 33. Zou, X.; Zhang, Y. Noble metal-free hydrogen evolution catalysts for water splitting. Chem. Soc. Rev. 2015, 44, 5148–5180. [CrossRef][PubMed] 34. Vesborg, P.C.K.; Seger, B.; Chorkendorff, I. Recent Development in Hydrogen Evolution Reaction Catalysts and Their Practical Implementation. J. Phys. Chem. Lett. 2015, 6, 951–957. [CrossRef][PubMed] 35. Hunt, S.T.; Nimmanwudipong, T.; Román-Leshkov, Y. Engineering Non-sintered, Metal-Terminated Tungsten Carbide Nanoparticles for Catalysis. Angew. Chem. Int. Ed. 2014, 53, 5131–5136. [CrossRef] Catalysts 2018, 8, 551 24 of 29
36. Wu, H.B.; Xia, B.Y.; Yu, L.; Yu, X.-Y.; Lou, X.W. Porous molybdenum carbide nano-octahedrons synthesized via conﬁned carburization in metal-organic frameworks for efﬁcient hydrogen production. Nat. Commun. 2015, 6, 6512. [CrossRef][PubMed] 37. Vrubel, H.; Hu, X. Molybdenum Boride and Carbide Catalyze Hydrogen Evolution in both Acidic and Basic Solutions. Angew. Chem. Int. Ed. 2012, 51, 12703–12706. [CrossRef][PubMed] 38. Chen, W.F.; Wang, C.H.; Sasaki, K.; Marinkovic, N.; Xu, W.; Muckerman, J.T.; Zhu, Y.; Adzic, R.R. Highly active and durable nanostructured molybdenum carbide electrocatalysts for hydrogen production. Energy Environ. Sci. 2013, 6, 943–951. [CrossRef] 39. Shi, Z.; Nie, K.; Shao, Z.-J.; Gao, B.; Lin, H.; Zhang, H.; Liu, B.; Wang, Y.; Zhang, Y.; Sun, X.; et al. [email protected] nanowires toward efﬁcient electrochemical hydrogen evolution: Composition, structural and electronic regulation. Energy Environ. Sci. 2017, 10, 1262–1271. [CrossRef] 40. Popczun, E.J.; McKone, J.R.; Read, C.G.; Biacchi, A.J.; Wiltrout, A.M.; Lewis, N.S.; Schaak, R.E. Nanostructured Nickel Phosphide as an Electrocatalyst for the Hydrogen Evolution Reaction. J. Am. Chem. Soc. 2013, 135, 9267–9270. [CrossRef][PubMed] 41. Chung, D.Y.; Jun, S.W.; Yoon, G.; Kim, H.; Yoo, J.M.; Lee, K.-S.; Kim, T.; Shin, H.; Sinha, A.K.; Kwon, S.G.; et al. Large-Scale Synthesis of Carbon-Shell-Coated FeP Nanoparticles for Robust Hydrogen Evolution Reaction Electrocatalyst. J. Am. Chem. Soc. 2017, 139, 6669–6674. [CrossRef][PubMed] 42. Huang, Z.; Chen, Z.; Chen, Z.; Lv, C.; Humphrey, M.G.; Zhang, C. Cobalt phosphide nanorods as an efﬁcient electrocatalyst for the hydrogen evolution reaction. Nano Energy 2014, 9, 373–382. [CrossRef] 43. Shi, Y.; Zhang, B. Recent advances in transition metal phosphide nanomaterials: Synthesis and applications in hydrogen evolution reaction. Chem. Soc. Rev. 2016, 45, 1529–1541. [CrossRef][PubMed] 44. McEnaney, J.M.; Chance Crompton, J.; Callejas, J.F.; Popczun, E.J.; Read, C.G.; Lewis, N.S.; Schaak, R.E. Electrocatalytic hydrogen evolution using amorphous tungsten phosphide nanoparticles. Chem. Commun. 2014, 50, 11026–11028. [CrossRef][PubMed] 45. McEnaney, J.M.; Crompton, J.C.; Callejas, J.F.; Popczun, E.J.; Biacchi, A.J.; Lewis, N.S.; Schaak, R.E. Amorphous Molybdenum Phosphide Nanoparticles for Electrocatalytic Hydrogen Evolution. Chem. Mater. 2014, 26, 4826–4831. [CrossRef] 46. Yin, J.; Fan, Q.; Li, Y.; Cheng, F.; Zhou, P.; Xi, P.; Sun, S. Ni–C–N Nanosheets as Catalyst for Hydrogen Evolution Reaction. J. Am. Chem. Soc. 2016, 138, 14546–14549. [CrossRef][PubMed] 47. Wang, Z.-L.; Hao, X.-F.; Jiang, Z.; Sun, X.-P.; Xu, D.; Wang, J.; Zhong, H.-X.; Meng, F.-L.; Zhang, X.-B. C and N Hybrid Coordination Derived Co–C–N Complex as a Highly Efﬁcient Electrocatalyst for Hydrogen Evolution Reaction. J. Am. Chem. Soc. 2015, 137, 15070–15073. [CrossRef][PubMed] 48. Zou, X.; Huang, X.; Goswami, A.; Silva, R.; Sathe, B.R.; Mikmeková, E.; Asefa, T. Cobalt-Embedded Nitrogen-Rich Carbon Nanotubes Efﬁciently Catalyze Hydrogen Evolution Reaction at All pH Values. Angew. Chem. Int. Ed. 2014, 53, 4372–4376. [CrossRef][PubMed] 49. Chianelli, R.R.; Siadati, M.H.; De la Rosa, M.P.; Berhault, G.; Wilcoxon, J.P.; Bearden, R.; Abrams, B.L. Catalytic Properties of Single Layers of Transition Metal Sulﬁde Catalytic Materials. Catal. Rev. 2006, 48, 1–41. [CrossRef] 50. Kisielowski, C.; Ramasse, Q.M.; Hansen, L.P.; Brorson, M.; Carlsson, A.; Molenbroek, A.M.; Topsøe, H.;
Helveg, S. Imaging MoS2 Nanocatalysts with Single-Atom Sensitivity. Angew. Chem. Int. Ed. 2010, 49, 2708–2710. [CrossRef][PubMed]
51. Tiwari, A.P.; Yoo, H.; Lee, J.; Kim, D.; Park, J.H.; Lee, H. Prevention of sulfur diffusion using MoS2-intercalated 3D-nanostructured graphite for high-performance lithium-ion batteries. Nanoscale 2015, 7, 11928–11933. [CrossRef][PubMed] 52. Huang, X.; Zeng, Z.; Zhang, H. Metal dichalcogenide nanosheets: Preparation, properties and applications. Chem. Soc. Rev. 2013, 42, 1934–1946. [CrossRef][PubMed] 53. Bonaccorso, F.; Lombardo, A.; Hasan, T.; Sun, Z.; Colombo, L.; Ferrari, A.C. Production and processing of graphene and 2d crystals. Mater. Today 2012, 15, 564–589. [CrossRef] 54. Kim, J.; Yoon, G.; Kim, J.; Yoon, H.; Baek, J.; Lee, J.H.; Kang, K.; Jeon, S. Extremely large, non-oxidized graphene ﬂakes based on spontaneous solvent insertion into graphite intercalation compounds. Carbon 2018, 139, 309–316. [CrossRef] Catalysts 2018, 8, 551 25 of 29
55. Novak, T.G.; Kim, J.; Song, S.H.; Jun, G.H.; Kim, H.; Jeong, M.S.; Jeon, S. Fast P3HT Exciton Dissociation and Absorption Enhancement of Organic Solar Cells by PEG-Functionalized Graphene Quantum Dots. Small 2016, 12, 994–999. [CrossRef][PubMed] 56. Park, K.H.; Kim, B.H.; Song, S.H.; Kwon, J.; Kong, B.S.; Kang, K.; Jeon, S. Exfoliation of Non-Oxidized Graphene Flakes for Scalable Conductive Film. Nano Lett. 2012, 12, 2871–2876. [CrossRef][PubMed]
57. Liu, N.; Kim, P.; Kim, J.H.; Ye, J.H.; Kim, S.; Lee, C.J. Large-Area Atomically Thin MoS2 Nanosheets Prepared Using Electrochemical Exfoliation. ACS Nano 2014, 8, 6902–6910. [CrossRef][PubMed] 58. Eunyoung, L.; Jinwook, B.; Ji Su, P.; Jin, K.; Jong Min, Y.; Seokwoo, J. Effect of nucleation density on the crystallinity of graphene grown from mobile hot-wire-assisted CVD. 2D Mater. 2019, 6, 011001. 59. Lee, J.; Baek, J.; Ryu, G.H.; Lee, M.J.; Oh, S.; Hong, S.K.; Kim, B.-H.; Lee, S.-H.; Cho, B.J.; Lee, Z.; et al. High-Angle Tilt Boundary Graphene Domain Recrystallized from Mobile Hot-Wire-Assisted Chemical Vapor Deposition System. Nano Lett. 2014, 14, 4352–4359. [CrossRef][PubMed] 60. Baek, J.; Novak, T.G.; Kim, H.; Lee, J.; Jang, B.; Lee, J.; Jeon, S. Analysis of contact resistance in single-walled carbon nanotube channel and graphene electrodes in a thin ﬁlm transistor. Nano Converg. 2017, 4, 35. [CrossRef][PubMed]
61. Chang, K.; Chen, W. l-Cysteine-Assisted Synthesis of Layered MoS2/Graphene Composites with Excellent Electrochemical Performances for Lithium Ion Batteries. ACS Nano 2011, 5, 4720–4728. [CrossRef][PubMed] 62. Guan, Z.; Ni, S.; Hu, S. Tunable Electronic and Optical Properties of Monolayer and Multilayer Janus MoSSe as a Photocatalyst for Solar Water Splitting: A First-Principles Study. J. Phys. Chem. C 2018, 122, 6209–6216. [CrossRef] 63. Tan, W.; Wei, Z.; Liu, X.; Liu, J.; Fang, X.; Fang, D.; Wang, X.; Wang, D.; Tang, J.; Fan, X. Ordered and Disordered Phases in Mo1−xWxS2 Monolayer. Sci. Rep. 2017, 7, 15124. [CrossRef][PubMed] 64. Tiwari, A.P.; Kim, D.; Kim, Y.; Prakash, O.; Lee, H. Highly active and stable layered ternary transition metal chalcogenide for hydrogen evolution reaction. Nano Energy 2016, 28, 366–372. [CrossRef] 65. Lu, A.-Y.; Zhu, H.; Xiao, J.; Chuu, C.-P.; Han, Y.; Chiu, M.-H.; Cheng, C.-C.; Yang, C.-W.; Wei, K.-H.; Yang, Y.; et al. Janus monolayers of transition metal dichalcogenides. Nat. Nanotechnol. 2017, 12, 744. [CrossRef] [PubMed] 66. Gong, Q.; Cheng, L.; Liu, C.; Zhang, M.; Feng, Q.; Ye, H.; Zeng, M.; Xie, L.; Liu, Z.; Li, Y. Ultrathin
MoS2(1–x)Se2x Alloy Nanoﬂakes For Electrocatalytic Hydrogen Evolution Reaction. ACS Catal. 2015, 5, 2213–2219. [CrossRef] 67. Xu, K.; Wang, F.; Wang, Z.; Zhan, X.; Wang, Q.; Cheng, Z.; Safdar, M.; He, J. Component-Controllable
WS2(1−x)Se2x Nanotubes for Efﬁcient Hydrogen Evolution Reaction. ACS Nano 2014, 8, 8468–8476. [CrossRef] [PubMed] 68. Song, S.H.; Kim, B.H.; Choe, D.-H.; Kim, J.; Kim, D.C.; Lee, D.J.; Kim, J.M.; Chang, K.J.; Jeon, S. Bandgap
Widening of Phase Quilted, 2D MoS2 by Oxidative Intercalation. Adv. Mater. 2015, 27, 3152–3158. [CrossRef] [PubMed]
69. Pruss, E.A.; Snyder, B.S.; Stacy, A.M. A New Layered Ternary Sulﬁde: Formation of Cu2WS4 by Reaction of WS and Cu+ Ions. Angew. Chem. Int. Ed. Eng. 1993, 32, 256–257. [CrossRef] 70. Hinnemann, B.; Moses, P.G.; Bonde, J.; Jørgensen, K.P.; Nielsen, J.H.; Horch, S.; Chorkendorff, I.; Nørskov, J.K.
Biomimetic Hydrogen Evolution: MoS2 Nanoparticles as Catalyst for Hydrogen Evolution. J. Am. Chem. Soc. 2005, 127, 5308–5309. [CrossRef][PubMed]
71. Tsai, C.; Chan, K.; Abild-Pedersen, F.; Nørskov, J.K. Active edge sites in MoSe2 and WSe2 catalysts for the hydrogen evolution reaction: A density functional study. Phys. Chem. Chem. Phys. 2014, 16, 13156–13164. [CrossRef][PubMed] 72. Lassalle-Kaiser, B.; Merki, D.; Vrubel, H.; Gul, S.; Yachandra, V.K.; Hu, X.; Yano, J. Evidence from in Situ X-ray Absorption Spectroscopy for the Involvement of Terminal Disulﬁde in the Reduction of Protons by an Amorphous Molybdenum Sulﬁde Electrocatalyst. J. Am. Chem. Soc. 2015, 137, 314–321. [CrossRef][PubMed] 73. Sun, T.; Wang, J.; Chi, X.; Lin, Y.; Chen, Z.; Ling, X.; Qiu, C.; Xu, Y.; Song, L.; Chen, W.; et al. Engineering
the Electronic Structure of MoS2 Nanorods by N and Mn Dopants for Ultra-Efﬁcient Hydrogen Production. ACS Catal. 2018, 8, 7585–7592. [CrossRef] 74. Xiao, W.; Liu, P.; Zhang, J.; Song, W.; Feng, Y.P.; Gao, D.; Ding, J. Dual-Functional N Dopants in Edges and
Basal Plane of MoS2 Nanosheets Toward Efﬁcient and Durable Hydrogen Evolution. Adv. Energy Mater. 2016, 7, 1602086. [CrossRef] Catalysts 2018, 8, 551 26 of 29
75. Han, X.; Tong, X.; Liu, X.; Chen, A.; Wen, X.; Yang, N.; Guo, X.-Y. Hydrogen Evolution Reaction on
Hybrid Catalysts of Vertical MoS2 Nanosheets and Hydrogenated Graphene. ACS Catal. 2018, 8, 1828–1836. [CrossRef]
76. Kumar, P.; Viswanath, B. Horizontally and vertically aligned growth of strained MoS2 layers with dissimilar wetting and catalytic behaviors. CrystEngComm 2017, 19, 5068–5078. [CrossRef] 77. Jaramillo, T.F.; Jørgensen, K.P.; Bonde, J.; Nielsen, J.H.; Horch, S.; Chorkendorff, I. Identiﬁcation of Active
Edge Sites for Electrochemical H2 Evolution from MoS2 Nanocatalysts. Science 2007, 317, 100–102. [CrossRef] [PubMed] 78. Tsai, C.; Chan, K.; Nørskov, J.K.; Abild-Pedersen, F. Theoretical insights into the hydrogen evolution activity of layered transition metal dichalcogenides. Surf. Sci. 2015, 640, 133–140. [CrossRef] 79. Yan, Y.; Xia, B.; Xu, Z.; Wang, X. Recent Development of Molybdenum Sulﬁdes as Advanced Electrocatalysts for Hydrogen Evolution Reaction. ACS Catal. 2014, 4, 1693–1705. [CrossRef] 80. Xie, J.; Zhang, J.; Li, S.; Grote, F.; Zhang, X.; Zhang, H.; Wang, R.; Lei, Y.; Pan, B.; Xie, Y. Controllable Disorder
Engineering in Oxygen-Incorporated MoS2 Ultrathin Nanosheets for Efﬁcient Hydrogen Evolution. J. Am. Chem. Soc. 2013, 135, 17881–17888. [CrossRef][PubMed]
81. Xie, J.; Zhang, H.; Li, S.; Wang, R.; Sun, X.; Zhou, M.; Zhou, J.; Lou, X.W.; Xie, Y. Defect-Rich MoS2 Ultrathin Nanosheets with Additional Active Edge Sites for Enhanced Electrocatalytic Hydrogen Evolution. Adv. Mater. 2013, 25, 5807–5813. [CrossRef][PubMed] 82. Laursen, A.B.; Kegnæs, S.; Dahl, S.; Chorkendorff, I. Molybdenum sulﬁdes—Efﬁcient and viable materials for electro—And photoelectrocatalytic hydrogen evolution. Energy Environ. Sci. 2012, 5, 5577–5591. [CrossRef]
83. Yu, Y.; Huang, S.-Y.; Li, Y.; Steinmann, S.N.; Yang, W.; Cao, L. Layer-Dependent Electrocatalysis of MoS2 for Hydrogen Evolution. Nano Lett. 2014, 14, 553–558. [CrossRef][PubMed]
84. Kibsgaard, J.; Chen, Z.; Reinecke, B.N.; Jaramillo, T.F. Engineering the surface structure of MoS2 to preferentially expose active edge sites for electrocatalysis. Nat. Mater. 2012, 11, 963. [CrossRef][PubMed]
85. Kong, D.; Wang, H.; Cha, J.J.; Pasta, M.; Koski, K.J.; Yao, J.; Cui, Y. Synthesis of MoS2 and MoSe2 Films with Vertically Aligned Layers. Nano Lett. 2013, 13, 1341–1347. [CrossRef][PubMed]
86. Tsai, C.; Abild-Pedersen, F.; Nørskov, J.K. Tuning the MoS2 Edge-Site Activity for Hydrogen Evolution via Support Interactions. Nano Lett. 2014, 14, 1381–1387. [CrossRef][PubMed]
87. Li, Y.; Wang, H.; Xie, L.; Liang, Y.; Hong, G.; Dai, H. MoS2 Nanoparticles Grown on Graphene: An Advanced Catalyst for the Hydrogen Evolution Reaction. J. Am. Chem. Soc. 2011, 133, 7296–7299. [CrossRef][PubMed] 88. Yang, J.; Voiry, D.; Ahn, S.J.; Kang, D.; Kim, A.Y.; Chhowalla, M.; Shin, H.S. Two-Dimensional Hybrid Nanosheets of Tungsten Disulﬁde and Reduced Graphene Oxide as Catalysts for Enhanced Hydrogen Evolution. Angew. Chem. Int. Ed. 2013, 52, 13751–13754. [CrossRef][PubMed] 89. Nai, J.; Lu, Y.; Yu, L.; Wang, X.; Lou, X.W. Formation of Ni–Fe Mixed Diselenide Nanocages as a Superior Oxygen Evolution Electrocatalyst. Adv. Mater. 2017, 29, 1703870. [CrossRef][PubMed] 90. Fang, M.; Dong, G.; Wei, R.; Ho, J.C. Hierarchical Nanostructures: Design for Sustainable Water Splitting. Adv. Energy Mater. 2017, 7, 1700559. [CrossRef] 91. Yu, L.; Yu, X.Y.; Lou, X.W. The Design and Synthesis of Hollow Micro-/Nanostructures: Present and Future Trends. Adv. Mater. 2018, 30, 1800939. [CrossRef][PubMed] 92. Nai, J.; Lou, X.W. Hollow Structures Based on Prussian Blue and Its Analogs for Electrochemical Energy Storage and Conversion. Adv. Mater. 2018, 1706825. [CrossRef][PubMed] 93. Deng, J.; Li, H.; Wang, S.; Ding, D.; Chen, M.; Liu, C.; Tian, Z.; Novoselov, K.S.; Ma, C.; Deng, D.; et al. Multiscale structural and electronic control of molybdenum disulﬁde foam for highly efﬁcient hydrogen production. Nat. Commun. 2017, 8, 14430. [CrossRef][PubMed] 94. Zhang, J.; Liu, S.; Liang, H.; Dong, R.; Feng, X. Hierarchical Transition-Metal Dichalcogenide Nanosheets for Enhanced Electrocatalytic Hydrogen Evolution. Adv. Mater. 2015, 27, 7426–7431. [CrossRef][PubMed]
95. Sun, L.; Wang, T.; Zhang, L.; Sun, Y.; Xu, K.; Dai, Z.; Ma, F. Mace-like hierarchical MoS2/NiCo2S4 composites supported by carbon ﬁber paper: An efﬁcient electrocatalyst for the hydrogen evolution reaction. J. Power Sources 2018, 377, 142–150. [CrossRef] 96. Liao, M.; Zeng, G.; Luo, T.; Jin, Z.; Wang, Y.; Kou, X.; Xiao, D. Three-dimensional coral-like cobalt selenide as an advanced electrocatalyst for highly efﬁcient oxygen evolution reaction. Electrochim. Acta 2016, 194, 59–66. [CrossRef] Catalysts 2018, 8, 551 27 of 29
97. Yu, X.-Y.; Yu, L.; Wu, H.B.; Lou, X.W. Formation of Nickel Sulﬁde Nanoframes from Metal–Organic Frameworks with Enhanced Pseudocapacitive and Electrocatalytic Properties. Angew. Chem. Int. Ed. 2015, 54, 5331–5335. [CrossRef][PubMed]
98. Yu, X.-Y.; Feng, Y.; Jeon, Y.; Guan, B.; Lou, X.W.; Paik, U. Formation of Ni–Co–MoS2 Nanoboxes with Enhanced Electrocatalytic Activity for Hydrogen Evolution. Adv. Mater. 2016, 28, 9006–9011. [CrossRef] [PubMed]
99. Liu, Y.; Zhang, J.; Li, Y.; Yuan, G.; Niu, X.; Zhang, X.; Wang, Q. Self-Templated Synthesis of Co1−xS Porous Hexagonal Microplates for Efﬁcient Electrocatalytic Oxygen Evolution. ChemElectroChem 2018, 5, 1167–1172. [CrossRef] 100. Kuang, M.; Wang, Q.; Han, P.; Zheng, G. Cu, Co-Embedded N-Enriched Mesoporous Carbon for Efﬁcient Oxygen Reduction and Hydrogen Evolution Reactions. Adv. Energy Mater. 2017, 7, 1700193. [CrossRef]
101. Ganesan, V.; Lim, S.; Kim, J. Hierarchical Nanoboxes Composed of Co9S8−MoS2 Nanosheets as Efﬁcient Electrocatalysts for the Hydrogen Evolution Reaction. Chem. Asian J. 2018, 13, 413–420. [CrossRef][PubMed] 102. Yu, L.; Xia, B.Y.; Wang, X.; Lou, X.W. General Formation of M–MoS3 (M = Co, Ni) Hollow Structures with Enhanced Electrocatalytic Activity for Hydrogen Evolution. Adv. Mater. 2015, 28, 92–97. [CrossRef] [PubMed] 103. Luo, Z.-M.; Wang, J.-W.; Tan, J.-B.; Zhang, Z.-M.; Lu, T.-B. Self-Template Synthesis of Co–Se–S–O Hierarchical Nanotubes as Efﬁcient Electrocatalysts for Oxygen Evolution under Alkaline and Neutral Conditions. ACS Appl. Mater. Interfaces 2018, 10, 8231–8237. [CrossRef][PubMed]
104. Zhou, W.; Lu, J.; Zhou, K.; Yang, L.; Ke, Y.; Tang, Z.; Chen, S. CoSe2 nanoparticles embedded defective carbon nanotubes derived from MOFs as efﬁcient electrocatalyst for hydrogen evolution reaction. Nano Energy 2016, 28, 143–150. [CrossRef] 105. Sun, J.; Chen, Y.; Ren, Z.; Fu, H.; Xiao, Y.; Wang, J.; Tian, G. Self-Supported NiS Nanoparticle-Coupled
Ni2P Nanoﬂake Array Architecture: An Advanced Catalyst for Electrochemical Hydrogen Evolution. ChemElectroChem 2017, 4, 1341–1348. [CrossRef] 106. Zhou, W.; Cao, X.; Zeng, Z.; Shi, W.; Zhu, Y.; Yan, Q.; Liu, H.; Wang, J.; Zhang, H. One-step synthesis of
Ni3S2 [email protected](OH)2 nanosheet core–shell nanostructures on a three-dimensional graphene network for high-performance supercapacitors. Energy Environ. Sci. 2013, 6, 2216–2221. [CrossRef]
107. Binjie, Z.; Yuanfu, C.; Fei, Q.; Xinqiang, W.; Wanli, Z.; Yanrong, L.; Xuesong, L. 3D-hierarchical MoSe2 nanoarchitecture as a highly efﬁcient electrocatalyst for hydrogen evolution. 2D Mater. 2017, 4, 025092. 108. Bian, L.; Gao, W.; Sun, J.; Han, M.; Li, F.; Gao, Z.; Shu, L.; Han, N.; Yang, Z.-X.; Song, A.; et al.
Phosphorus-Doped MoS2 Nanosheets Supported on Carbon Cloths as Efﬁcient Hydrogen-Generation Electrocatalysts. ChemCatChem 2017, 10, 1571–1577. [CrossRef] 109. Zhang, X.; Li, J.; Yang, Y.; Zhang, S.; Zhu, H.; Zhu, X.; Xing, H.; Zhang, Y.; Huang, B.; Guo, S.; et al.
Co3O4/Fe0.33Co0.66P Interface Nanowire for Enhancing Water Oxidation Catalysis at High Current Density. Adv. Mater. 2018, 1803551. [CrossRef][PubMed]
110. Wu, M.; Huang, Y.; Cheng, X.; Geng, X.; Tang, Q.; You, Y.; Yu, Y.; Zhou, R.; Xu, J. Arrays of ZnSe/MoSe2 Nanotubes with Electronic Modulation as Efﬁcient Electrocatalysts for Hydrogen Evolution Reaction. Adv. Mater. Interfaces 2017, 4, 1700948. [CrossRef]
111. Li, H.; Yu, K.; Tang, Z.; Zhu, Z. Experimental and First-Principles Investigation of MoWS2 with High Hydrogen Evolution Performance. ACS Appl. Mater. Interfaces 2016, 8, 29442–29451. [CrossRef][PubMed] 112. Zhou, X.; Jiang, J.; Ding, T.; Zhang, J.; Pan, B.; Zuo, J.; Yang, Q. Fast colloidal synthesis of scalable Mo-rich
hierarchical ultrathin MoSe2−x nanosheets for high-performance hydrogen evolution. Nanoscale 2014, 6, 11046–11051. [CrossRef][PubMed] 113. Lai, J.; Niu, W.; Luque, R.; Xu, G. Solvothermal synthesis of metal nanocrystals and their applications. Nano Today 2015, 10, 240–267. [CrossRef]
114. Tao, L.; Duan, X.; Wang, C.; Duan, X.; Wang, S. Plasma-engineered MoS2 thin-ﬁlm as an efﬁcient electrocatalyst for hydrogen evolution reaction. Chem. Commun. 2015, 51, 7470–7473. [CrossRef][PubMed] 115. Zhang, X.; Meng, F.; Mao, S.; Ding, Q.; Shearer, M.J.; Faber, M.S.; Chen, J.; Hamers, R.J.; Jin, S. Amorphous MoSxCly electrocatalyst supported by vertical graphene for efﬁcient electrochemical and photoelectrochemical hydrogen generation. Energy Environ. Sci. 2015, 8, 862–868. [CrossRef]
116. Tang, H.; Dou, K.; Kaun, C.-C.; Kuang, Q.; Yang, S. MoSe2 nanosheets and their graphene hybrids: Synthesis, characterization and hydrogen evolution reaction studies. J. Mater. Chem. A 2014, 2, 360–364. [CrossRef] Catalysts 2018, 8, 551 28 of 29
117. Zhou, H.; Yu, F.; Huang, Y.; Sun, J.; Zhu, Z.; Nielsen, R.J.; He, R.; Bao, J.; Goddard Iii, W.A.; Chen, S.; et al. Efﬁcient hydrogen evolution by ternary molybdenum sulfoselenide particles on self-standing porous nickel diselenide foam. Nat. Commun. 2016, 7, 12765. [CrossRef][PubMed] 118. Li, F.; Wei, W.; Zhao, P.; Huang, B.; Dai, Y. Electronic and Optical Properties of Pristine and Vertical and Lateral Heterostructures of Janus MoSSe and WSSe. J. Phys. Chem. Lett. 2017, 8, 5959–5965. [CrossRef] [PubMed] 119. Konkena, B.; Masa, J.; Xia, W.; Muhler, M.; Schuhmann, W. [email protected] graphene oxide nanocomposite heterostructures as efﬁcient and stable electrocatalysts for the hydrogen evolution reaction. Nano Energy 2016, 29, 46–53. [CrossRef] 120. Kosmala, T.; Coy Diaz, H.; Komsa, H.-P.; Ma, Y.; Krasheninnikov, A.V.; Batzill, M.; Agnoli, S. Metallic Twin Boundaries Boost the Hydrogen Evolution Reaction on the Basal Plane of Molybdenum Selenotellurides. Adv. Energy Mater. 2018, 8, 1800031. [CrossRef] 121. Putungan, D.B.; Lin, S.-H.; Kuo, J.-L. A ﬁrst-principles examination of conducting monolayer 1T’-MX2 (M = Mo, W; X = S, Se, Te): Promising catalysts for hydrogen evolution reaction and its enhancement by strain. Phys. Chem. Chem. Phys. 2015, 17, 21702–21708. [CrossRef][PubMed] 122. Gholamvand, Z.; McAteer, D.; Backes, C.; McEvoy, N.; Harvey, A.; Berner, N.C.; Hanlon, D.; Bradley, C.;
Godwin, I.; Rovetta, A.; et al. Comparison of liquid exfoliated transition metal dichalcogenides reveals MoSe2 to be the most effective hydrogen evolution catalyst. Nanoscale 2016, 8, 5737–5749. [CrossRef][PubMed] 123. Sun, C.; Zhang, J.; Ma, J.; Liu, P.; Gao, D.; Tao, K.; Xue, D. N-doped WS2 nanosheets: A high-performance electrocatalyst for the hydrogen evolution reaction. J. Mater. Chem. A 2016, 4, 11234–11238. [CrossRef] 124. Liu, P.; Zhu, J.; Zhang, J.; Xi, P.; Tao, K.; Gao, D.; Xue, D. P Dopants Triggered New Basal Plane Active Sites
and Enlarged Interlayer Spacing in MoS2 Nanosheets toward Electrocatalytic Hydrogen Evolution. ACS Energy Lett. 2017, 2, 745–752. [CrossRef] 125. Er, D.; Ye, H.; Frey, N.C.; Kumar, H.; Lou, J.; Shenoy, V.B. Prediction of Enhanced Catalytic Activity for Hydrogen Evolution Reaction in Janus Transition Metal Dichalcogenides. Nano Lett. 2018, 18, 3943–3949. [CrossRef][PubMed] 126. Tan, S.M.; Pumera, M. Composition-Graded MoWSx Hybrids with Tailored Catalytic Activity by Bipolar Electrochemistry. ACS Appl. Mater. Interfaces 2017, 9, 41955–41964. [CrossRef][PubMed] 127. Li, C.; Bo, X.; Li, M.; Guo, L. Facile electrodeposition fabrication of molybdenum-tungsten sulﬁde on carbon cloth for electrocatalytic hydrogen evolution. Int. J. Hydrogen Energy 2017, 42, 15479–15488. [CrossRef] 128. Gan, X.; Lv, R.; Wang, X.; Zhang, Z.; Fujisawa, K.; Lei, Y.; Huang, Z.-H.; Terrones, M.; Kang, F. Pyrolytic carbon supported alloying metal dichalcogenides as free-standing electrodes for efﬁcient hydrogen evolution. Carbon 2018, 132, 512–519. [CrossRef] 129. Shi, Y.; Zhou, Y.; Yang, D.-R.; Xu, W.-X.; Wang, C.; Wang, F.-B.; Xu, J.-J.; Xia, X.-H.; Chen, H.-Y. Energy Level
Engineering of MoS2 by Transition-Metal Doping for Accelerating Hydrogen Evolution Reaction. J. Am. Chem. Soc. 2017, 139, 15479–15485. [CrossRef][PubMed] 130. Chua, X.J.; Luxa, J.; Eng, A.Y.S.; Tan, S.M.; Sofer, Z.; Pumera, M. Negative Electrocatalytic Effects of p-Doping
Niobium and Tantalum on MoS2 and WS2 for the Hydrogen Evolution Reaction and Oxygen Reduction Reaction. ACS Catal. 2016, 6, 5724–5734. [CrossRef] 131. Lukowski, M.A.; Daniel, A.S.; Meng, F.; Forticaux, A.; Li, L.; Jin, S. Enhanced Hydrogen Evolution Catalysis
from Chemically Exfoliated Metallic MoS2 Nanosheets. J. Am. Chem. Soc. 2013, 135, 10274–10277. [CrossRef] [PubMed]
132. Ambrosi, A.; Sofer, Z.; Pumera, M. 2H → 1T phase transition and hydrogen evolution activity of MoS2, MoSe2, WS2 and WSe2 strongly depends on the MX2 composition. Chem. Commun. 2015, 51, 8450–8453. [CrossRef][PubMed]
133. Tsai, C.; Chan, K.; Nørskov, J.K.; Abild-Pedersen, F. Rational design of MoS2 catalysts: Tuning the structure and activity via transition metal doping. Catal. Sci. Technol. 2015, 5, 246–253. [CrossRef] 134. Askari, M.B.; Beheshti-Marnani, A.; Banizi, Z.T.; Seiﬁ, M.; Ramezan Zadeh, M.H. Synthesis and evaluation of MoWCoS/G and MoWCuS/G as new transition metal dichalcogenide nanocatalysts for electrochemical hydrogen evolution reaction. Chem. Phys. Lett. 2018, 691, 243–249. [CrossRef] 135. Zhan, F.; Wang, Q.; Li, Y.; Bo, X.; Wang, Q.; Gao, F.; Zhao, C. Low-Temperature Synthesis of Cuboid Silver
Tetrathiotungstate (Ag2WS4) as Electrocatalyst for Hydrogen Evolution Reaction. Inorg. Chem. 2018, 57, 5791–5800. [CrossRef][PubMed] Catalysts 2018, 8, 551 29 of 29
136. Zhou, X.; Lin, S.-H.; Yang, X.; Li, H.; Hedhili, M.N.; Li, L.-J.; Zhang, W.; Shi, Y. MoSx-coated NbS2 nanoﬂakes grown on glass carbon: An advanced electrocatalyst for the hydrogen evolution reaction. Nanoscale 2018, 10, 3444–3450. [CrossRef][PubMed] 137. Tiwari, A.P.; Azam, A.; Novak, T.G.; Prakash, O.; Jeon, S. Chemical strain formation through anion
substitution in Cu2WS4 for efﬁcient electrocatalysis of water dissociation. J. Mater. Chem. A 2018, 6, 7786–7793. [CrossRef] 138. Kim, Y.; Tiwari, A.P.; Prakash, O.; Lee, H. Activation of Ternary Transition Metal Chalcogenide Basal Planes through Chemical Strain for the Hydrogen Evolution Reaction. ChemPlusChem 2017, 82, 785–791. [CrossRef]
139. Gong, Q.; Sheng, S.; Ye, H.; Han, N.; Cheng, L.; Li, Y. MoxW1−x(SySe1−y)2 Alloy Nanoﬂakes for High-Performance Electrocatalytic Hydrogen Evolution. Part. Part. Syst. Charact. 2016, 33, 576–582. [CrossRef] 140. Wang, F.; Sun, Y.; He, Y.; Liu, L.; Xu, J.; Zhao, X.; Yin, G.; Zhang, L.; Li, S.; Mao, Q.; et al. Highly efﬁcient and durable MoNiNC catalyst for hydrogen evolution reaction. Nano Energy 2017, 37, 1–6. [CrossRef]
© 2018 by the authors. Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (http://creativecommons.org/licenses/by/4.0/).